OPTIMISATION OF DESIGN OF COMPOSITE STRUCTURES
Antonio Miravete
WOODHEAD PUBLISHING LIMITED
OPTIMISATION OF DESIGN O...
270 downloads
1053 Views
10MB Size
Report
This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!
Report copyright / DMCA form
OPTIMISATION OF DESIGN OF COMPOSITE STRUCTURES
Antonio Miravete
WOODHEAD PUBLISHING LIMITED
OPTIMISATION OF DESIGN OF COMPOSITE STRUCTURES
OPTIMISATION OF DESIGN OF COMPOSITE STRUCTURES
Antonio Miravete Department of Mechanical Engineering University of Zaragoza
WOODHEAD PUBLISHING LIMITED
Cambridge England
Published by Woodhead Publishing Limited, Abington Hall, Abington, Cambridge CB21 6AH, England www.woodheadpublishing.com First published 1996 © Woodhead Publishing Ltd, 1996
Conditions of sale All rights reserved. No part of this publication may be reproduced or transmitted in any form or by any means, electronic or mechanical, including photocopy, recording, or any information storage and retrieval system, without permission in writing from the publisher. British Library Cataloguing in Publication Data A catalogue record for this book is available from the British Library. ISBN13: 9781855732087 ISBNlO: 1855732084 Printed by Victoire Press, Cambridge, England.
CONTENTS
Preface Symbols and notation 1 Introduction and preliminaries
Vll
viii 1
1.1 Introduction
1
1.2 Anisotropic constitutive relations
2
1.3 Laminate theories
7
1.4 Numerical methods of stress analysis
11
1.5 Failure criteria
13
1.6 Numerical methods for design optimisation
14
References
16
2 Design optimisation of constant thickness composite structures
19
2.1 Introduction
19
2.2 Special configurations: SMC and fabric composites
21
2.3 Homogenisation of laminated plates
29
2.4 The freeedge effect
31
2.5 Conclusions
34
References
35
3 Shells
39
3.1 Introduction
39
3.2 Spherical dome
39
3.3 Spherical vessel
46
3.4 Pipeline and submersible hull
51
3.5 Conclusions
55
References
56
4 Constant thickness plates
59
4.1 Introduction
59
4.2 Design optimisation of composite plates in bending
59
4.3 Design optimisation of composite plates in buckling
71
4.4 Conclusions
81
References
83
5 Constant thickness sandwiches
87
5.1 Introduction
87
5.2 Core materials
87
5.3 Optimum design of sandwich constructions
98
5.4 Buckling
105
5.5 Conclusions
113
References
114
6 Design optimisation of variable thickness composite structures
117
6.1 Introduction
117
6.2 Variable thickness laminate stress distribution
118
6.3 Conclusions
135
References
135
7 Variable thickness beams
137
7.1 Introduction
137
7.2 Behaviour of variable thickness composite beams
138
7.3 Optimisation of variable thickness composite beams
148
7.4 Conclusions
152
References
153
8 Variable thickness plates
155
8.1 Introduction
155
8.2 Model assumptions and method of analysis
155
8.3 Determination of elastic constants and strengths
158
8.4 Optimisation of laminated composite plates
160
8.5 Conclusions
181
References
182
9 Variable thickness sandwiches
185
9.1 Introduction
185
9.2 Onedimensional laminated composite panels
186
9.3 Twodimensional laminated composite panels
188
9.4 Conclusions
198
References
199
PREFACE Composite materials have been increasingly used during the last decades, to lighten structures in fields such as aeronautics and space. Two steps are essential to take advantage of these materials: design and optimisation. Optimisation of composite structures is a recent issue, because both optimisation techniques and composite structures have been developed during the last few decades and therefore, the conjunction of them is even more recent. As using composite materials is an expensive but efficient way of getting minimum weight structures, it is logical to attempt to find out how to design properly optimised laminated composite plates with no reduction in their strength. Since many kinds of ground and air vehicles have rectangular plates as a common structural element, an increasing demand for improved structural efficiency in such applications has resulted. Composite materials offer a number of advantages other than their high stiffness to density values: for example, it is possible to shape them by orientating the filaments in the various layers in order to optimise the desired structural behaviour. Although there is much literature related to plate analysis, the most modem references lack adequate information which could allow a designer to tailor or synthesise an optimal design. There are two reasons for this: llfstly, the difficulty of accurately assessing the level of strains and stresses in any point of a laminated composite plate and, secondly, the need to implement an optimisation procedure able to find the minimum weight structure. Fortunately, the current development of numerical techniques and the existence of powerful computers provide a solution to the two problems mentioned above. Recently, a number of books dealing with design on composite materials have been published. This is the llfst step for relating theory of composite materials to real life, the objective being to produce information that can be used for design purposes. The aim of this book is to provide another step forward and to obtain rules, not only to design composite structures properly but to do this in an optimum way. Two software packages are included with the book for designing and optimising rectangular, constant and variable thickness composite plates. The author wishes to express his gratitude to Steve W Tsai and Ran Y Kim, for their encouragement and support in the course of the work related to variable thickness structures. The support of the Mechanics and Surface Interactions Branch (WRDCIMLBM), Nonmetallic Material Division, Materials Laboratory, Wright Research and Development Center, Wright Patterson Air Force Base, Ohio, USA is also acknowledged. Special thanks are due to Juan J Alba, Maria J Casamayor, Luis Castej6n, Javier Fernandez and Jesus Saldafia, who are all members of the Group of Composite Materials of the University of Zaragoza. Finally I wish to express my appreciation to Teresa Laborde who was in charge of editing text and graphics.
Antonio Miravete
vii
Symbols and notation
a
Length of the plate; or nodal displacement vector
a'
Relative nodal displacement Nodal displacement vector of the finite element e
B
Geometric matrix used in the [mite element method; B = L N
b
Width of the plate
CIJ
Stiffness matrix in the generalized Hooke's law; in concentrated notation, i,j=1,2,3,4,5,6
c
Straindisplacement matrix, or core thickness in a sandwich panel
D
Matrix of elastic constants
E
Young modulus
eIJ
Strain energy of the jth layer of the element i
eIJ
Strain energy density of the jth layer of the element i
e'
Strain energy density of the jth layer of the element i
e'IJ
Relative strain energy of the jth layer of the element i
IJ
Strength parameters in stress formulation of the quadratic failure criterion Nodal forces in the [mite element e Inplane shear modulus
hO
Ply thickness
K
Stiffness matrix of the whole plate
K'
Relative stiffness matrix of the whole plate Stiffness matrix of the whole plate due to bending stresses Geometric matrix of the whole plate Elemental stiffness matrix Diagonal of a plate
II
Surface area of the element i
M
Applied bending moment
N
Shape function matrix Applied compressive force in xdirection per unit width Critical compressive force in xdirection per unit width
viii
Applied compressive force in ydirection per unit width Critical compressive force in ydirection per unit width Applied compressive force in xy or 12plane per unit width Critical compressive force in xy or 12plane per unit width P
Applied transverse load
Q
Reduced stiffness matrix for plane stress
cf
Distributed forces in the [mite element e Term of the reduced matrix for plane stress Qyy =By / (1v12v21)
r
Strength/stress ratio or strength ratio
S
Positive pure shear strength in the xy or 12plane of a ply
S'
Negative pure shear strength in the xy or 12plane of a ply
T
Transformation matrix Total laminate thickness Difference between the total laminate thickness (t) and the minor thickness of a tapered plate
t·· 1J
Thickness of the jth layer of the ith element
u
Deflection in the xdirection
Y
Strain energy of a single plate element subjected to inplane stresses Strain energy of a single plate element due to plate bending Yolume of the finite element e
Y·· 1J
Yolume of the jth layer of the ith element Strain energy of a single plate element due to inplane stresses
v
Deflection in the y direction
w
Deflection in the zdirection
x
Uniaxial tensile strength of a ply along the x axis
X'
Uniaxial compressive strength of a ply along the xaxis
Y
Uniaxial tensile strength of a ply along the yaxis
Y'
Uniaxial compressive strength of a ply along the yaxis
Z
Uniaxial tensile strength of a ply along the zaxis
Z'
Uniaxial compressive strength of a ply along the zaxis
a··1J
Thickness of the jth layer of the ith element normalized to maximum thickness
"{ ..
1J
Shear strain component Strain generated by a virtual displacement ix
Su
Displacement generated by a virtual displacement
se
Vector of nodal deflections
Sae
Virtual displacements in the fmite element e
101
Strain component
E'i
Relative strain component
EO
Initial strains
e
Angle between x axis and fiber or principal axis of layer
A
Scaling parameter
A
Lagrangian parameter; or coefficient used to formulate an eigenvalue problem
v
Number of cycle of iteration
Angle of variation of thickness
Pij
Mass density of the jth layer of the ith element
(j1
Stress component
(j'i
Relative stress component
(jo
Initial stresses
't 1J
Shear stress component
..... A
2>.
2!..
Onedimensional thin plate Onedimensional thick plate
Onedimensional sandwich plate Onedimensional simply supported plate
Onedimensional clamped plate
Onedimensional cantilever plate
Twodimensional thin plate
Twodimensional thick plate
Twodimensional sandwich plate
Twodimensional simply supported plate
x
Twodimensional clamped plate
111111
IS.
A
1
h
Onedimensional plate subjected to a uniform transverse load
A
Onedimensional plate subjected to a point transverse load
Twodimensional plate subjected to a uniform transverse load
Twodimensional plate subjected to a point transverse load
o
Onedimensional simply supported plate
'   _ _ _...r.~
Onedimensional clamped plate
D o
Onedimensional cantilever plate
Twodimensional simply supported plate
Twodimensional simply supported plate
Twodimensional plate subjected to a uniaxial uniform compression load
xi
LIIIIIIIl
101 ttttttttt
Twodimensional plate subjected to a biaxial uniform compression load (Ny=N x /2)
111111111
101 ttttttttt
• 101 • IDI ~
Twodimensional plate subjected to a biaxial uniform compression load (Ny=Nx)
Twodimensional plate subjected to a biaxial uniform compression load (Ny=Nx *2)
Twodimensional plate subjected to a uniform inplane shear load
Twodimensional plate subjected to a uniaxial uniform compression and inplane shear load
xii
1 INTRODUCTION AND PRELIMINARIES Designing with composite materials is complex because there are many variables to consider: orientation of fibres, number of plies, ply thickness, type of fibre, type of matrix, configuration, etc. Thus, the optimum design is not obvious and different cases must be considered. The chapters of this book fall into three groups. Chapter 1 provides a general background on composite materials: anisotropic constitutive relations, laminated plates and shear theories to be applied to thin and thick laminates, respectively. Chapters 2 to 5 are concerned with constant thickness composite structures, and provide a survey of various design methodologies of shells, plates and sandwich constructions. Chapters 6 to 9 examine variable thickness composite structures, and consider beams, plates and sandwiches. The users' manuals of DAC and OPT!, two software packages for designing constant and variable thickness structures respectively, are presented separately. First of all, constant thickness structures are studied. Shells, plates and sandwiches are analysed in terms of design optimisation, the weight being the optimisation criterion. Different applications are reviewed and a comparison with standard materials and optimum configurations is given for each case. Secondly, variable thickness structures are studied. Beams, plates and sandwiches are analysed and a comparison with constant thickness structures and optimum configurations is given for each case. 1.1. Introduction The aim of this chapter is to define the basis of the analyses described in this book. First, anisotropic constitutive relations are presented in order to obtain the stressstrain relations for composite materials. Then, the formulation of two theories which are the most widely used in the field of composites design is described. These are the laminated plate theory and the frrst order shear theory. The laminated plate theory is simple and easy to implement. The results obtained by means of this theory are accurate for thin plates (characteristic length/thickness> 10). Thus, this theory is very useful for this type of plate because several optimisation criteria for design may be easily obtained. When wolking with thick plates (characteristic length/thickness < 10), the interlaminar effect cannot be neglected and thus, a shear theory must be used. For design optimisation pwposes, the first order shear theory gives good results and therefore, that methodology will be used in this book. To obtain very accurate results, a higher order shear theory is more adequate. A rational basis of structural engineering design must be based on the ability to predict the load and hence, the stress, likely to be encountered in practice. Therefore, a numerical method to carry out the stress analyses in an optimum way must be selected.
I
Failure criteria are needed for design optimisation and materials improvement. The most frequently used criteria are extensions of similar criteria for isotropic materials, which include those for maximum stress, maximum strain and quadratic. The choice of an appropriate failure criterion is made in this chapter. Finally, the numerical methods applied in this text for optimisation purposes are described.
1.2 Anisotropic constitutive relations Laminated composites are constructed from orthotropic plies containing collimated unidirectional fibres, woven cloth or chopped strand mattings. Generally, in a macroscopic sense, the lamina is assumed to behave as a homogeneous orthotropic material. The constitutive relation for a linear elastic orthotropic material in the fibre coordinate system, Fig. 1.1, is (13): tl
Sl1
S12
S13
0
0
0
t2
S12
S22
S23
0
0
0
0'2
t3
S13
S23
S33
0
0
0
0'3
1 23
0
0
0
S44
0
0
't 23
131
0
0
0
0
S55
0
't 31
112
0
0
0
0
0
S66
0'1
't 12
[1.1]
where the stress components (OJ. 'tij) are defined in Fig. 1.1 and Sij are elements of the compliance matrix. The strain components
(~}
'Yij) are defined in a manner analogous to the stress components.
In a thin lamina a plane stress is commonly assumed by setting: [1.2]
a3
1
a
1
Figure 1.1 Defmition of stress components and principal material directions for an orthotropic material.
2
For equation 1.1 this assumption leads to:
[1.3]
123 = 131 = 0
Thus, £3 is not an independent strain component and does not need to be included in the constitutive relationship for plane stress. Equation 1.1 becomes:
c1
Su
S12
0
<J 1
c2
S12
S22
0
<J2
112
0
0
S66
't 12
[1.4]
Sij may be related to the engineering constants as:
[1.5] The relation in equation 1.4 may be inverted to obtain the stress components from the strain components: <J 1
Qll
Q12
0
c1
<J2
Q12
Q22
0
c2
't 12
0
0
Q66
112
[1.6]
where Q.j are the reduced stiffnesses:
= E/ (1 Q12 = '\)12Ei Q ll

'\)12'\)21)
(1  '\)12'\)21)
Q22 = Ei (1 
'\)12'\)21)
Q 66 = G 12
[1.7]
For a lamina whose principal material axes are oriented at an angle with respect to the x  y system (see Fig. 1.2), the stresses and strains transform according to:
"{"xy
[1.8]
and 3
= [T] [1.9] where the transformation matrix is:
2mn
[T] =
2mn [1.10]
z,3 2
x Figure 1.2 Positive rotation of principal material axes (12) from arbitrary xy axes. in which m=cose [1.11]
n = sine
From equations 1.8 and 1.9 it is possible to establish the stressstrain relation in any coordinate system. In this way the compliance relation becomes:
ex ty
=
Su
S12
S16
S12
S22
S26
S16
S26
S66
ax ay
'xy
'(xv
[1.12]
4
Similarly, the stiffness relation becomes:
O"x O"y
=
1'xy
0 11 012 0 16
tx
0 12 022 026
ty
0 16 022 066
Yxy [1.13]
where the bars denote transfOlmed properties obtained from:
Sll = m 4S 11
= S22 = S21
S12
+ m 2n 2 (2S 12 + S66 ) + n 4S22
=
m 2n 2 (Sll + S22  S66 )
+ S12 (m4 + n 4 )
n 4S 11 + m 2n 2 (2S 12 + S66 ) + m 4S 22
[1.14]
S16 = 2m 3n (Sll  S12)
+ 2mn3 (S12  S22)
mn (m 2 _n 2 )S66
S26 = 2mn3 (Sll  S12)
+ 2m 3n (S12  S22)
+ mn (m 2  n2)S66
2 4m 2n 2 (S 12  S) 22 + (m ·_ n2)2S66
Q ll = m4Qll Q 21 = Q 12
+ 2m 2n 2 (Q12 + 2Q66)
=
+ n4Q22
m 2n 2 (Qll + Q 22  4Q66) + (m4 + n 4) Q 12
Q 22 = n4Qll + 2m 2n 2 (Q12 + 2Q66)
+ m4Q22
Q16 = m 3n (Qll  Q12) + mn3 (Q12  Q22)  2mn (m 2  n 2)Q66 Q26 = mn3 (Qll  Q12) + m 3n (Q12  Q22) +2mn (m 2  n 2)Q66 Q 66 = m 2n 2 (Qll + Q 22  2Q12  2Q66) + (m 4 + n4)Q 66
[1.15]
Hygrothermal strains. As fibrous composite materials are processed at elevated temperatures, thermal strains introduced during cooldown to room temperature may lead to residual stresses and changes in dimensions. Furthermore, matrices may be hygroscopic and tend to absorb moisture which may lead to swelling strains and stresses in the material. The constitutive relationship with temperature and swelling strains included takes the following form:
O"X O"y 1'xy
=
0 11 0 12 0 16
ex
0 12 022 026
ty
0 16 022 066
Yxy [1.16]
5
CX Cy
=
S11
S12
S16
S12
S22
S16
S16
S26
S66
tT x
O'x O'y
tT y
+
Txy
Yxy
CSx
+
T
t Sy
'("~y
Yxy
where superscripts T and S denote temperature and swellinginduced strains, respectively. Inversion of equation 1.16 gives:
O'x O'y
=
Txy
0 11 0 12 0 16
Cx
_t T x
_t S x
012 022 026
Cy
_c T
tSxy
016 026
Yxy
Yxy
066
Y
T
'fxy [1.17]
The thermal and swelling strains may in many cases be expressed as linear functions of the temperature and the moisture concentration:
cx. x
[1.18]
cS ~y
L\C
R
Py
[1.19]
where AT and AC are the temperature change and moisture concentration change from the reference state. As might be expected, transformations for expansional strains are similar to those for mechanical strains (equation 1.9). Note that in the principal material coordinate system: [1.20] as no shear strain is introduced in the principal coordinate system because of a change in temperature or moisture concentration. In many cases, only the steady state temperature and moisture concentration in the composite is of interest. For this case, AT and AC are constants throughout the material. However, in a transient situation, the transfer of heat by
6
conduction or diffusion of water has to be considered. There is an obvious analogy between the two phenomena that was first recognised by Fick who developed a mathematical formalism for diffusion, similar to heat transfer.
1.3 Laminate theories
1.3.1 Laminated plates theory The basic assumptions for the laminated plates theory 117 are: 1
The plate is constructed of an arbitrary number of layers of orthotropic sheets bonded together. However, the orthotropic axes of material symmetry of an individual layer need not coincide with the xy axes of the plate.
2
The plate is thin, i.e., the thickness h is much smaller than the other physical dimensions.
3
The displacements u, v, and w are small compared with the plate thickness.
4
Inplane strains ex, loy and exy are small compared with unity.
5
In order to include inplane force effects, nonlinear terms in the equations of motion involving products of stresses and plate slopes are retained. All other nonlinear terms are neglected.
6
Transverse shear strains exz and eyz are negligible.
7 Tangential displacements u and v are linear functions of the z coordinate. 8 The transverse normal strain ez is negligible. 9 Each ply obeys Hook's law. 10 The plate has constant thickness. 11 Rotary inertia terms are negligible. 12 There are no body forces. 13 Transverse shear stresses O"xz and O"yz vanish on the surfaces z = ± h/2. A laminate is made up of a number of plies with an arbitrary planar orientation (see Fig. 1.3). For the displacements of the crosssection of the laminate, it is assumed that a line, originally straight and perpendicular to the middle surface, remains so during deformation. This assumption leads to the vanishing of the outofplane shear strains: [1.21]
Yxz = Yyz = 0 where the laminate coordinate system (x  y  z) is indicated in Fig. 1.3.
Moreover, the strain ez in the thickness direction is neglected. Consequently, the laminate strains are reduced to ex' loy' and Yxy' by the above assumptions, which constitute the Kirchhoff hypothesis for plates. Assuming that the crosssections undergo only stretching and rotation leads to the following strain distribution,
7
to x
tx ty
Kx
to y
=
Yxy
Ky
z
+
0
Kxy
Yxy
[1.22]
where (cOx' EO y' YOxy) and (Kx ' K y' Kxy) are the midplane strains and curvatures, respectively, and z is the distance from the midplane.
x Figure 1.3 Laminate coordinate system. The resultant forces and moments are obtained by integration of the stresses in each layer over the laminate thickness,
h: Nx
cr x hl2
Ny N xy
= J
h/2
cry
dz
'fxy k
[1.23]
cr x
Mx h/2
My Mxy
= J
h/2
cry
zdz
'fxy k
[1.24]
where (Nx' Ny' N xy ) and (Mx' My' Mxy) are the force and moment resultants, respectively. The subscript k represents the kth lamina in the laminate. Combination of equations 1.17 to 1.19, 1.22 to 1.24 leads to:
8
Nx
=
Ny N xy
A12
A16
A12
A,.2
A,.6
A 16
A,.6
~6
CO x CO
+
Y
°
Yxy
Bu
B12
B16
Kx
B12
B22
B 26
Ky
B 16
B 26
B66
Kxy: [1.25]
Mx
=
My
Au
Mxy
BU
B12
B16
CO x
B12
B22
B 26
CO y
B16
B 26
B66
Yxy
+
°
DU
D12
D16
Kx
D12
D22
D 26
Ky
D16
D 26
Do6
Kxy: [1.26]
Aij. Bij and Dij are called extensional stiffnesses, coupling stiffnesses, and bending stiffnesses, respectively. They are calculated from: N
L
A..
IJ
(Qij)k
(~ ~)
k=l
N
B ..
IJ
=
1 2
L
(Qij)k
(~

~l)
k=l N
D .. IJ
1
3
L
(Qij)k (zi  zil)
k=l
[1.27]
1.3.2 First order shear theory For composites having a high ratio of inplane Young's moduli to interlaminar shear moduli and ratios of inplane dimensions to thickness less than ten, significant differences between the exact solutions and results from classical theory are observed. In particular, maximum plate deflections are shown to be considerably larger than predicted by classical laminated plate theory. As a result it is appropriate to develop a fIrst order laminated plate theory which can be applied to moderately thick plates. There are several references related to shear theories (1827). In this section a shear theory (Whitney 18) which includes the effects of transverse shear deformation and rotary inertia is considered. Solutions to the theory are also presented for the purpose of assessing the effect of transverse shear deformation on the behaviour of laminated plates. The approach presented is an extension of theories developed by Reissner and Mindlin for homogeneous, isotropic plates to laminates consisting of an arbitrary number of bonded anisotropic layers. Such an extension was originally due to Yang, Norris, and Stavsky with some later modification by Whitney and Pagano. 1.3.2.1 Constitutive equations The basic assumptions for the shear deformation theory are:
9
1 The plate is constructed of an arbitrary number of layers of orthotropic sheets bonded together. However, the orthotropic axes of material symmetry of an individual layer need not coincide with the xy axes of the plate. 2
The plate is thin, i.e., the thickness h is much smaller than the other physical dimensions.
3
The displacements u, v, and w are small compared with the plate thickness.
4
Inplane strains tx, ty and txy are small compared with unity.
5
In order to include inplane force effects, nonlinear terms in the equations of motion involving products of stresses and plate slopes are retained. All other nonlinear terms are ignored
6 Tangential displacements u and v are linear functions of the z coordinate. 7 The transverse normal strain tz is negligible. 8 Each ply obeys Hook's law. 9 The plate has constant thickness. 10 There are no body forces. 11 Transverse shear stresses 0xz and Oyz vanish on the surfaces z = + hl2. Thus the displacements are now assumed to be of the form:
u = UO(x,y,t) + z'l'x(x,y,t)
v = VO(x,y,t) + z'l'y(x,y,t) W
= w(x,y,t)
[1.28]
Using equation 1.28 in conjunction with the straindisplacement relations:
[1.29]
The following results are obtained:
[1.30]
where the mid plane strains are defined in the usual manner, by the equation:
°
avo
E =Y
ay
° =auO +avo
E
xy
ay
ax
10
and
[1.31] In addition, the interlaminar shear strains are given by the relationships:
[1.32] Using equation 1.30 in conjunction with the assumption of plane stress within each ply, equation 1.22, and the deftnition of force and moment resultants, equations 1.23 and 1.24, a constitutive relation of exactly the same form as given by equations 1.25 and 1.26 can be obtained, i.e. in abbreviated notation:
[1.33]
where the stiffness terms Ai} Bij, and Dij are defined by equation 1.27. Applying the definition of shear force resultants, we obtain an additional constitutive relation involving transverse shear. Following Reissner and Mindlin we introduce a parameter k in this constitutive relation for transverse shear. Thus we obtain:
[1.34] where Eyz and Exz are defmed in equation 1.32 and h/2
A .. = 1J
fe. .dz 1J
(i,j = 4,5)
h/2
[1.35]
with the Cij terms denoting anisotropic stiffnesses. Values associated with the factor k may be obtained in the literature. 28 1.4 Numerical methods of stress analysis Although in a few cases boundary element methods have been used, the bulk of a considerable body of literature uses the fmite element method. 2934 Thus, the analyses of the structures studied in this text have been carried out by means of the ftnite element method. By means of this technique, strains and stresses can be obtained in any point of the plate. With the finite element method, the interior of the plate is idealised as an assembly of discrete elements over which the unknown displacements are represented approximately by linear, quadratic, etc, variations. Thus, the governing equation of internal equilibrium is satisfied approximately. 11
Let Oae be a virtual displacement of the nodes. This displacement generates the following displacements inside the finite element: Ou= N
oae
[1.36]
and the following strains inside the finite element: [1.37] The work done by the node forces is equal to the addition of the products of each component of force by the corresponding displacement [1.38] Analogously, the internal worknormalised to volumedone by distributed stresses and forces is [1.39] or [l.40]
The external work must be equal to the internal work integrated on the elemental volume. Therefore,
[1.41]
This expression is valid for any virtual displacement. Thus,
[1.42] For a linear relationship between stresses and strains, the following expression can be obtained: [1.43] where k e is the elemental stiffness matrix:
[1.44] and
[1.45] 12
The forcedisplacement relation for the whole plate is given by:
[1.46]
[K] {a} = {q}
where [K] is the stiffness matrix of the structure, {a} is the displacement vector, and {q} is the force vector. The strain energy eij of the jth layer of the ith element is given by:
[1.47] The element strains {£} i in the ith element are expressed by:
[1.48]
{Eh = [c] {ali
where [c] is the straindisplacement matrix. The stresses {a hj in the jth layer of the ith element are given by:
[1.49] where [Q]ij is the matrix of elastic constants of the jth layer of the ith element
1.5 Failure criteria For optimisation processes, the concept of the strength/stress ratio is extremely useful. Thus, the chosen failure criterion must have a unique strength/stress ratio for each combined state of stress and the corresponding state of strain. Owing to this, a quadratic criterion has been applied. According to Tsai and Wu,35 there exists a failure surface in the stressspace in the following scalar form: i,j
= 1,2,3,4,5,6
[1.50]
where the contracted notation is used; Fi and Fij are strength tensors of the second and fourth rank, respectively. One method of applying the strength criterion is to transform the stress components into the materialsymmetry axes. The final expression will be composed by the following terms:
Fl aI' + F2 (a2' + a3') + Fll' a 1'2 + F22' (a 2'2 +a 3'2 + 2 a 4'2 ) + F66 (a 5'2 +a 6'2) + 2 F12 (aI' a2' + aI' a3')+ 2F23(a2' a3' + a 4'2) = 1
[1.51]
where
Fl = l/Xl/X'
[1.52]
Fl1 = 1I(X X')
[1.53]
F2 = ININ'
[1.54]
=1I(Y Y') =1I(Z Z') = 1I(S S')
[1.55]
F22 F33 F66
[1.56] [1.57]
13
The coupling or interaction terms can be calculated by means of the following formula: p..
p ..
IJ = IJ
and
* [ p11.. pJJ..
]112
i#j
[1.58]
Pij * =  0.5
[1.59]
The strength/stress ratio r is the ratio between the maximum, ultimate or allowable strength, and the applied stress: {cr}max. =r {cr} applied
[1.60]
Since each combination of stress components in equation 1.50 reaches its maximum when the lefthand side reaches unity, we can substitute equation 1.60 into: p.. IJ cr·1 cr·J + F1 cr·1 1
[1.61]
.. cr· cr· ] r2 + [F1cr·] r  1  0 [p IJIJ 1
[1.62]
Ifwedefme [1.63] [1.64] Then, the strength/stress ratio r is the positive square root in the quadratic formula: r
=( b /2a ) + [( b /2a )2+ 1Ia ] 112
[1.65]
1.6 Numerical methods for design optimisation The recurrence relations proposed here for resizing the elements for variable thickness structures are based on the optimality criteria, which are not rigorous in the mathematical sense, but are found to give near optimum weight designs for large structures in an efficient way. The optimality criterion for the generalised stiffness requirement can be stated as, "the optimum structure is the one in which the ratio of the average strain energy density to the mass density is the same in all the elements" .36 This criterion can be written as: 1 
)..
e··IJ / p IJ.. [1.66]
where).. is the Lagrangian parameter,
e ij is the strain energy density of the jth layer of the ith element, and Pij is the
mass density. The strain energy density is given by: [1.67]
14
where Vij is the volume of the element defmed by:
v··IJ = t,· '1J
11
[1.68]
where tij is the thickness of the jth layer of the ith element and Ii is the surface area of the ith element. The design variable tij can be written as: [1.69] where O:ij is the relative thickness (normalised to the maximum thickness) of the jth layer of the ith element, and A is the scaling parameter. Introducing the scaling parameter in equation 1.46 gives: A [K'] {a} = {q}
[1.70]
or
={q}
[1.71]
{a} = {a'} I A
[1.72]
[K'] {a'}
where
and [K'] is the stiffness matrix for the whole structure obtained by using the relative design vector O:ij Introducing the scaling parameter into equations 1.47 to 1.49, the relations between the actual quantities and the relative quantities at element level can be expressed as:
=A [k'hj
[khj
[1.73]
{ah= {a'h/A
[1.74]
{Eh={E'h /A
[1.75]
{crhj = {cr'hj I A
[1.76]
where the prime quantities are the relative values. Introducing equations 1.67, 1.73 and 1.74 into equation 1.66 gives: e'ij
e'··IJ I (A2
1  A.
pIJ .. )
[1.77]
where
e'··IJ 
{r'}t.1 [K']··IJ {r'}·1 1(0:·· IJ 1·) 1
[1.78]
2 Multiplying both sides of equation 1.77 by O:ij and taking the square root gives: 0:..
IJ


B 0: .. (e'·· I p.. )112 IJ
IJ
[1.79]
IJ
where B is a constant Equation 1.79 can be rewritten in an iterative form as:
15
[1.80] where v and v+ 1 refer to the cycles of iteration. In this procedure the resizing of an element is achieved by dividing the design variable by the minimum actual strength/stress ratio for that element: (a. ij )v+l
=
[1.81]
(a. ij)v / (r)min v
Therefore, the election of the appropriate failure criterion is critical. If the strength/stress ratio defmed by the failure criterion is unique for each combined state of stress and the corresponding state of strain, the application of equation 1.81 is efficient and simple. Otherwise, the application of the procedure becomes more complicated. For constant thickness structures, sensitivity studies are usually applied to obtain optima configurations. Other optimisation procedures are also available. 37 51 References
1
Ashton J E, Halpin J C and Petit P H, Primer on Composite Materials; Analysis, Westport, Connecticut, Technomic, 1969.
2
Jones R M., Mechanics of Composite Materials, McGrawHill, New York, 1975.
3
Withney J M ,Daniel I M and Pipes R B, Experimental Mechanics of Fiber Reinforced Composite Materials, PrenticeHall, Englewood Cliffs, New Jersey, 1984.
4
Stavsky Y , 'Thermoelasticity of heterogeneous allotropic plates', J Eng Mech Diy. vol 89, no EM 2 1963, 89.
5
Halpin J C and Pagano N J , 'Consequences of Environmentally Induced Dilatation in Solids' in Recent Advances in Eng Sci, vol 5 (1970), p 3.
6
Whitney J M and Ashton J E , Effect of environment on the elastic response of layered composite plates', AlAA 1. vol 9, no 9, 1970, 1708.
7
Ozisik M N , Heat Conduction, Wiley, New York, 1980.
8
Springer G S, (ed.) Environmental Effects on Composite Materials, Technomic,Westport, Connecticut, 1981.
9
Pipes R B , Vinson J R and Chou T W , 'On the hygrothermal response of laminated composite systems', I Comp Mat 1976, 10, 129.
10
Carlsson LA, 'Outofplane hygroinstability of multiply paperboard', Fibre Sci and Tech, 1981, 14,201.
11
Timoshenko S P and Goodier J N , Theory of Elasticity. 3rd ed McGrawHill, New Yolk, 1970.
12
Horgan C 0, 'Some remarks on SaintVenant's principle for transversely isotropic composites', J Elasticity, 1972, 2, 335.
13
Choi I and Horgan CO, 'SaintVenant's Principle and End Effects in Anisotropic Elasticity', J App Mech, vol 44 (1977), P 424.
14
Horgan CO 'SaintVenant's end effects in composites', J Camp Mat 1982, 16,411.
16
15
Carlsson LA, Sindelar P and Nilsson S, Decay of end effects in graphite/epoxy bolted joints', Compo Sci. Tech, 1986,26,307.
16
Arridge R G C,Barham P I ,Farell C J and Keller A , 'The importance of end effects in the measurement of moduli of highly anisotropic materials', J Mater Sci, 1976, 11, 788,
17
Carlsson LA, Pipes R B , Experimental characterisation of advanced composite materials', Prentice Hall, Inc New York, 1987,
18
Lo, K H, Christensen, R M, Wu, E M, 'A high order theory of plate deformation part I: Homogeneous plates', ASME, J Appl Mech, 1977,44,663.
19
Lo, K H, Christensen, R M, Wu, EM, 'A high order theory of plate deformation part II: Laminated plates', ASME, J Appl Mech. 1977, 44, 669.
20
Reissner, E, 'On transverse bending of plates, including the effects of transverse shear deformation', Int J Solids Struct, 1975, 11, 569,
21
Kant T, Owen D R J, Zienkiewicz 0 C, 'A refined higher order Co plate bending element', Comput Struct, 1982, 15, 77.
22
Reddy J N, 'A simple higher order theory for laminated composite plates', ASME J Appl Mech, 1984, 51, 745.
23
Pandya B N, Kant T, 'A refined higherorder generally orthotropic Co plate bending element', Comput Struct 1988, 28, 119.
24
Laksminarayana H V, Ramani T S, 'On improving the performance of a shearflexible triangular laminated composite plate finite element' , Proc Int Conf Com Mat and Struct, Madras, 1988.
25
Prathap G, Somashekar BR, 'A fieldconsistent 8noded laminated anisotropic plate element', Proc Int Conf Com Mat and Struct, Madras, 1988.
26
Tessler A, 'An improved higherorder theory for orthotropic plates', Proc RevMech Comp, Bal Harbour, Florida, 1988.
27
Miravete A, 'A Simple Finite Element Formulation for ThreeDimensional Laminated Composite Plates', Proc5th Conf Comp Struct, Paisley, Scotland, 1989.
28
Withney J M, 'Shear correction factors of orthotropic laminates under static load', ASME J Appl. Mechanics, 1973, 40, 302304. .
29
Zienkiewicz 0 C, Taylor R L and Too J M, 'Reduced integration techniques in general analysis of plates and shells', Int J Num Meth Engng, 1971, 3, 275.
30
Pawsey S E, Clough R W, 'Improved numerical integration of thick shell finite elements', Int J Num Meth Engng, 1971, 3, 545.
31
Hughes T J R, Taylor R L and Kanoknukulchal W, 'A simple and efficient finite element for plate bending', Int J Num Meth Engng, Vo1l1, 1529, 1977
32
Pugh, E D L, Hinton, E and Zienkiewicz, 0 C, 'A study of quadrilateral plate bending with reduced integration', Int J Num Meth Engng, 1978, 12, 1059.
33
Lee S Wand Pian T H, 'Improvement of plate and shell finite elements by mixed formulations', AIAA J, 1978, 16, 29.
34
Hughes T J R and Tezduyar T E, 'Finite Elements based upon Mindlin platetheory, with particular reference to the fournode bilinear.
35
Tsai S W and Wu E M, 'A general theory of strength for anisotropic materials', J Comp, Mat, 1971, 5, 58.
17
36
Khot N S, Venkayya V B and Berke L, 'Optimum design of structures with stress and displacement constraints', AIAA, 14, pp1311322, 1976.
37
Donaldson S, 'Simplified weight saving techniques for composite panels', J Reinf Plastics and Composites, 1983.
38
Wurzel D P, 'On the optimal design of bidirectional composites', AFWALTR834060, Air Force Materials Laboratory, 1983
39
Massard T N, 'Computer sizing of composite laminates for strength', J Reinf Plastics and composites, 1984, 3,300.
40
Maksimovic S, 'Optimum design of composite structures', Proc 3rd Conf Comp Struct, Paisley, pp 148, 1985
41
Tsai S W, Composites design, (ed. Tsai, S W, Massard, TN, Susuki, I), 1985
42
Watkins R I, Morris A J, 'A multicriteria objective function optimization scheme for laminated composites for use in multilevel structural optimization schemes', Comp Meth in Em: 1987,233.
43
Iyengar N G R, 'Optimal design of fiber reinforced composite plates', Proc Advances in Aerospace structures, Madras, pp 71, 1988.
44
Pedersen P, 'On Optimal orientation of Orthotropic Materials', (inpress).
45
Leissa A W, 'Buckling of laminated composite plates and shell panels', AFW ALTR853069, Airforce Materials Laboratory, 1985.
46
Muc A, 'Optimal fibre orientation for simplysupported, angleply plates under biaxial compression', Comp Struct, 1988, 9, 161.
47
Reissner E and Stavsky Y, ASME J Appl Mech 1961, 28, 83),402.
48
Timoshenko S P and WoinowskyKrieger S, 'Theory of plates and shells', McGraw Hill, New York, 1959
49
Cook R D, 'Concepts and Applications of Finite Element Analysis', John Wiley, New York, 1981.
50
Reissner E, 'The effect of transverse shear deformation on the bending of elastic plates', ASME J Awl Mech 1945, 12, A69A77.
51
Mindlin R D, 'Influence of rotatory inertia and shear deformation on flexural motions of isotropiC elastic plates', ASME J Appl Mech.
18
2 DESIGN OPTIMISATION OF CONSTANT THICKNESS COMPOSITE STRUCTURES 2.1 Introduction Unlike variable thickness composites where stress concentration effects in the area of change of thickness are critical, constant thickness composites design is related to the global behaviour of the structure, particularly stiffness and strength. Firstly, stiffness and strength properties of some composite material systems are presented. Next, special configurations like SMC and fabric composites are analysed and micromechanical formulations given so as to obtain the ply stiffness and strength parameters as a function of fibre and matrix properties. Also, a comparison study between a fabric and a [0/90] configuration is carried out in order to fmd out whether a fabric can be modelled as two unidirectional plies. The behaviour of balanced and unbalanced fabrics is studied. Balanced fabrics (same amount of fibres in the two principal directions of the fabric) have seen most use in industrial applications. Square plates subjected to transverse uniform load must be designed with balanced fabrics. However, nonsquare plates should not be designed with such a configuration; nonbalanced fabrics must be used. The homogenisation of laminated plates is also analysed. When the number of repetitions is higher than ten, the laminate behaves as a homogeneous material and can be treated as an orthotropic nonlaminated material. Finally, the free edge effect is studied from the point of view of design optimisation Different solutions are described for minimising the delaminate process on laminated composite materials. Design optimisation of some constant thickness composite structures like shells, plates and sandwich constructions is analysed in Chapters 3  5. Composite materials embrace a wide range of reinforcing fibres, such as boron, glass, carbon and aramid. Advanced composite materials are used mostly in the form of preimpregnated sheets which consist of a number of aligned unidirectional rovings impregnated with an epoxy resin matrix. In this form a variety of structural materials can be made by stacking plies in different directions in much the same way as plywood. With these variations in ply orientation, stiffness and strength properties change and, as a consequence, a large number of laminate configurations need evaluation. Some stiffness and strength properties for advanced composite materials have been included in Table 2.1.1 Studies on the effect of different laminate orientations and layups have reduced somewhat the number of configurations that are likely to be used for structural members, and this has Simplified the collection of design data. Glass fibre is a comparatively cheap fibre with a high specific strength (see Table 2.2)2 and has seen extensive commercial utilisation in the form of chopped strand matting (Table 2.3)2 and woven roving (WR) (Table 2.4).2
19
Table 2.1 Stiffness and strength properties of boron, carbon and aramid fibres composite materials.
Type Fibre Matrix
CFRP T300 N5208
v/f(%) 70 ho,mm 0.125 Density 1.60 Ply stiffnessiGPa) 181.00 Ex 20.30 Ey 0.28 Vx 7.17 Es StrenJl;th (MPa) X 1500 X' 1500 Y 40 Y' 246 S 68
BFRP B(4) N5505
CFRP AS 3501
KFRP Kev49 epoxy
50 0.125 2.00
66 0.125 1.60
204.00 18.50 0.23 5.59 1260 2500 61 202 67
CFRP HIM6 epoxy
60 0.125 1.46
CFRTP AS4 PEEK APC2 66 0.125 1.60
CCRP T300 F934 13mil 60 0.325 1.50
CCRP
66 0.125 1.60
CFRP T300 F934 4mil 60 0.100 1.50
138.00 8.96 0.30 7.10
76.00 5.50 0.24 2.30
134.00 8.90 0.28 5.10
203.00 11.20 0.32 8.40
148.00 9.65 0.30 4.55
74.00 74.00 0.05 4.55
66.00 66.00 0.04 4.10
1447 1447 52 206 93
1400 235 12 53 34
2130 1100 80 200 160
3500 1540 56 150 98
1314 1220 43 168 48
499 352 458 352 46
375 279 368 278 46
TIOO F934 7mil 60 0.175 1.50
Table 2.2 Stiffness and strength properties of unidirectional fibre glass composite materials
Type Fibre Matrix v/f(%) ho, mm Density Ply stiffness (GPa) Ex Ey Vx Es StrenJl;th (MPa) X X' Y Y'
S
GFRP UnidR600 Epoxy 65.31 1.00 2.082
GRFP UnidR1200 Epoxy 69.67 1.00 2.141
GFRP UnidE1200 Vinylester 40.23 0.44 1.674
GFRP UnidE500 Polyester 51.85 0.49 1.926
GFRP UnidEglass Epoxy 45.00 0.25 1.800
57.100 15.067 0.3020 5.032
60.830 19.865 0.2955 6.517
31.161 7.452 0.3397 2.738
39.296 10.289 0.3222 4.260
38.60 8.27 0.26 4.14
1300.0 1100.0 80.0 70.0 75.00
1600.0 1400.0 70.0 65.0 70.00
500.0 500.0 50.0 50.0 50.00
1000.0 900.0 60.0 60.0 65.00
1062.0 610.0 31.0 118.0 72.0
20
Table 2.3 Stiffness and strength properties of fibre glass fabrics composite materials
Type Fibre Matrix v/f(%) ho, mm Density Ply stiffness. (GPa) Ex Ey Vx Es Strenl?;th (MPa) X X' y y' S
GFRP FabE500A Polyester 27.41 0.70 1.584
GFRP FabE500B Polyester 31.58 0.61 1.642
GFRP FabE580 Polyester 40.91 0.55 1.773
GFRP FabE600 Polyester 40.91 0.56 1.773
GFRP FabE50OC Vinylester 48.51 0.40 1.802
GFRP FabE500D Polyester 31.58 0.61 1.642
14.440 13.639 0.1480 2.070
16.228 15.312 0.1415 2.260
19.817 19.817 0.1309 2.781
20.065 19.569 0.1326 2.781
9.320 36.960 0.0825 3.347
16.228 15.312 0.1415 2.260
196.0 196.0 180.0 180.0 45.00
400.0 400.0 380.0 380.0 40.00
185.0 180.0 180.0 1750 45.00
185.0 180.0 180.0 175.0 45.00
350.0 350.0 320.0 320.0 45.00
200.0 160.0 200.0 160.0 50.00
Table 2.4 Stiffness and strength properties of chopped strand matting fibre glass composite materials. Type Fibre Matrix v/f(%) ho, mm Density Ply stiffness (GPa) Ex Ey Vx Es Strenl?;th (MPa) X X' y y' S
GFRP CSME600A Polyester 16.51 1.40 1.431
GFRP CSME300 Polyester 23.53 0.49 0.529
GFRP CSME600B Vinylester 37.72 0.61 1.635
GFRP CSMUnifllo Vinylester 35.94 0.48 1.607
7.733 7.733 0.3426 2.880
9.771 9.771 0.3354 3.659
14.236 14.236 0.3287 5.357
13.641 13.641 0.3292 5.131
100.0 100.0 100.0 100.0 30.00
140.0 140.0 140.0 140.0 30.00
160.0 150.0 160.0 160.0 30.00
180.0 180.0 180.0 180.0 30.00
2.2 Special configurations: SMC and fabric composites
2.2.1 Short fibre composites Short fibre composites include sheet moulding composites (SMC) and whisker composites. Using laminated plate theory, we can derive: • The Qisotropic constants for randomly oriented fibres in the plate can be obtained using the plane stress constants mentioned before.
21
• The Qisotropic strengths can be obtained using the [1t/3] Qisotropic laminates subjected to uniaxial tensile and compressive stresses, and pure shear, together with the quadratic failure criterion . • The strength is based on the lastplyfailure (LPF) on the assumption that the SMC strength reaches its ultimate at LPF. The Tresca and Mises criteria can be modified to predict the shear strength. Sensitivity of the fibre volume on the SMC strength will also be shown. The cost effectiveness in terms of fibre volume can then be predicted accordingly. Tsai3 has modelled the SMC configuration by using the Qisotropic constants (see Table 2.5): Table 2.5 Modelling of SMC by means of the Qisotropic constants Type Fibre Matrix
CFRP T300 N5208
BFRP B(4) N5505
59.66 16.96 21.35
20.54 5.51 7.47
32.44 10.54 10.95
57.04 17.28 19.88
85.88 25.43 30.23
CFRP T300 F934 4mil .taI>e 62.47 19.73 21.37
54.84 0.28 21.35
18.96 0.27 7.47
29.02 0.32 10.95
51.81 0.30 19.88
78.35 0.30 30.23
56.24 0.32 21.37
CFRP AS 3501
Linear combinations of [Q], GPa U1* 76.37 87.70 22.61 28.36 U4* U5* 26.88 29.67 * invariant Qisotropic constants E,GPa 69.68 78.53 nu 0.30 0.32 G,GPa 26.88 29.67
GFRP Eglass epoxy
KFRP Kev49 epOxy
CFRTP AS 4 PEEK APC2
CFRP HIM6 epOXY
CCRP T300 F934 13mil cloth 58.84 19.05 29.89
52.67 0.32 19.89
CCRP
TIOO F934 7mil cloth 52.37 16.66 17.85
47.0 0.32 17.8
Qisotropic constants are defmed as follows:
E iso
=[1 
V iS02 ]U l' v iso
= ~4 ,GiSO = U 5
[2.1]
1
The micromechanics formulas for SMC (Eglass/epoxy SMC) are given by the empirical model by Manera and Massot:
E =[16E +2Em ]= v +Em 8 45
f
f
[2.2]
9
G =[2E 3 ]=v +Em 1 +Em 15 4 3 f
[2.3]
f
_ e v=1
[2.4]
2G
This formula for isotropic media is not reliable because the ratio of E over G is close to one. Error is magnified when one is subtracted from this ratio. The strength is given by the following expression:
x
= 510v f +14
[2.5]
22
2.2.2 Woven composites Woven composites are intended to cover fabric, as well as structures made by filament winding and braiding. Since fibres must cross over, laminated plate theory that is applicable to discrete plies in a multidirectional laminate must be modified. The author is not aware of any simple theory that can predict the stiffness and strength of woven composites. The simplest way is to use a [0/90] laminate of the same ply material to model a balanced woven fabric. For unbalanced fabrics, the ratio between the 0 and 90 degree plies can match that between the warp and fill yarns. The difficulties in taking account of the fibre cross over arise from the loss of stiffness and strength along the fibres. When fibres are not straight their effective stiffness will reduce. Their tensile strength will reduce because of the additional bending stress and contact stress at cross over points. The compressive strength will also reduce because fibres are more prone to buckling. Another factor that causes difficulty is the fibre volume fraction, which is not likely to be as unifolTIl as that for cross ply composites. Voids are also more likely to occur near the cross over points. A comparison between the stiffness and strength of a [0/90] composite and those of a balanced fabric made from the same composite material has been shown by Tsai3 (Table 2.6). While the fibre volume fractions are only comparable, the use of cross ply to model fabric is accurate within 20% for glass and kevlar composites. However for graphite composites which have stiff fibres the model is not accurate. For the purpose of design, it is best to use the experimentally measured fabric data directly, replacing the ply data of a unidirectional composite. Further development of the model for the fibre cross over will include the degraded fibre stiffness and strength. 2.2.2.1 Comparison of [0/90] and woven fabric The predictions of elastic constants of fabrics, filamentwound and braided structures can be made if it is possible to replace the woven composite by a multidirectional laminate consisting of the same fibre angles and ply group ratios. Only then can the micromechanics fOlTIlulas for stiffness be applied to the plies without modification. In Table 2.6, three ply materials are compared to see how close [0/90] laminates can represent balanced woven fabrics of the same fibres and fibre volume fractions. Thus, under each of the three ply materials, the first column lists the engineering constants of the unidirectional ply. In the second column, the predicted effective laminate stiffness of a [0/90] crossply laminate are listed. The predicted values are indicated by an asterisk. These laminate stiffnesses can be compared with those measured from a balanced woven fabric or cloth, listed in the third column. The same bases of comparison apply to the other two ply materials. For the stiffnesses in the x and ydirections, the [0/90] laminate is higher than those measured from the fabric. This is not unexpected when the fibres in the fabric are not straight, and is true for graphite and kevlar/epoxy composites. The laminate stiffness is 19 and 14% higher than the fabric stiffness, respectively. In the case of the glass/epoxy composite, the laminate stiffness is 18% less than the fabric stiffness. There was apparently a difference in the fibre volume fractions that may account for the lower laminate stiffness. The Poisson's ratio and shear moduli of the [0/90] laminates are close to those of the fabrics. The predicted strengths of [0/90] are also compared with corresponding strengths measured from fabrics in the table below. With only one exception the compressive strength of glassepoxy fabric, crossply laminates have higher strengths than the fabrics. This is not unexpected because the fibres in fabrics are bent. The fibres in contact will cause local stress concentrations that would reduce tensile strengths. Bent fibres reduce buckling strengths which, in turn, reduce compressive strengths. 23
Table 2.6 Comparison of [0/90] and woven fabrics for carbon, glass and aramid fibre composites
Type Fibre Matrix
Stiffness (GPa) Ex Ey v/x Es Strel!Kths (MPa) X X' Y y' S
GrapJh'lte/ epoxy CFRP CCRP CCRP T300 T300 T300 F934 F934 F934 [0] [0/90] tape laminate cloth
E l f ,epoxy ~Jass kev lar49/epoxy KFRP KFRP KCRP GFRP GFRP GCRP Eglass E~lass F161 kev49 kev49 kev49 epoxy epoxy N5209 epoxy epoxy 6581 [0/90] ro/90] [01 ro1 tape tape laminate cloth laminate cloth
148.00 9.65 0.30 4.55
79.2* 79.2* 0.04* 4.6*
66.00 66.00 0.04 4.10
38.60 8.27 0.26 4.14
23.6* 23.6* 0.09* 4.1 *
29.6 26.9 0.12 6.24
76.00 5.50 0.34 2.30
41.0* 41.0* 0.05* 2.3*
35.8 35.8 0.09 1.79
1314 1220 43 168 48
664 899 664 899 49*
375 279 368 278 46
1062 610 31 118
545* 306* 545* 306* 80*
489 390 444 305 133
1400 235 12 53 34
704* 165* 704* 165* 34*
582 189 582 189 84
72
* Predicted values 2.2.2.2 Balanced and unbalanced fabrics Though both balanced and unbalanced fabrics are available, most fabrics used in engineering applications are balanced. This configuration is recommended only in those cases, where values of stresses in 0 0 and 90 0 directions are very similar. If there is a significant difference between values of stresses in 0 0 and 900 directions, unbalanced fabrics must be used. Let us consider a rectangular plate (thickness: t, length: a and width: b) subjected to transverse uniform load (q). By means of the theory described in Chapter 1, the deflection of the plate is given by the following expression: [2.6] Figures 2.1 and 2.2 show the deflection (value of k) of a fibreglass/epoxy resin rectangular plate, simply supported and clamped along the four edges, respectively. In both cases, the maximum deflection is given by balanced configurations for nonsquare plates. The next deflection is given by lightly unbalanced configurations (60% of fibres in the transverse direction and 40% in the longitudinal direction) and so on. The stiffest plate is composed of an unbalanced configuration (100% of fibres in the transverse direction): k = 0.18 and k = 0.9 for a plate with b > 2.5 a, and clamped and simply supported along the four edges, respectively. For a balanced configuration: k = 0.36 and k= 1.8 for a plate with b > 2.5 a, and clamped and simply supported along the four edges, respectively. Thus, a narrow plate (b > 2.5 a), composed of a balanced configuration presents a double deflection with respect to the optimum configuration (an unbalanced configuration, 100% fibres in the transverse direction). For narrow plates, the deflection decreases linearly with the percentage of fibres in the transverse direction. For square plates, there are slight differences between the five configurations represented in Fig. 2.1 and 2.2. The optimum one corresponds to a balanced configuration.
24
Another finding is the big difference between deflections of simplysupported and clamped plates. There is a factor of 5.
0.4
0,35
...........•.................
.
.~..
 ......
~ ....~ ..~
. .  ..
~.. ~ .. ~
I ~aucr~o:u~ ~~~~
0,3
,(
.
0,25
•
____ [50%]
•
0[60%] k 0,2
. ...
  . _.         _.
+[80%] ~[100%]
0,15
0,1
0,05
.  _ ..  _.               
.. ....... ..... ...•..........
2
. .............. .
3
5
4
alb
Figure 2.1 TIOO15208, rectangular plate, all clamped edges, uniform load. {(Opl90qhols; p + q = 5.
2
........ .
1,8
.
•...... ... ............... ....• ....

1,6
1,4
____ [50%] 0[60%] k 1
+[80%] .     .  .t •.. ______ . _ . . ____ . ______ . . . . ____________ . . _ . _________ . ____ . __ . . __ _
0,8
~[100%]
0,6
. . . . . . . . ...
................................................     ' ............................. .
0,4
   _.   _... _.  _.     _.        _.  .,  _.               .. 
0.2
._ .       _..                           .   _..
2
_. _..    .   ..    _. .   .  _...
4
3
5
alb
Figure 2.2 TIOO15208, rectangular plate, all supported edges, uniform load {(Opl90qhols; p + q =5. 25
In both cases, the maximum deflection is given by balanced configurations for nonsquare plates. The next deflection is
given by lightly unbalanced configurations (60% of fibres in the transverse direction and 40% in the longitudinal direction) and so on. Similar conclusions are obtained for aramid fibre composite plates. The stiffest plate is composed of an unbalanced configuration (100% of fibres in the transverse direction): k = 0.22 and k= 1.15 for a plate with b > 2.5 a, and clamped and simply supported along the four edges, respectively (Fig. 2.3 and 2.4). For a balanced configuration: k = 0.44 and k= 2.30 for a plate with b> 2.5 a, and clamped and simply supported along the four edges, respectively.
0:: I.•.. 0,4
··7. ~ . ~u..... ....
... ;
_
TU.T
.T
••
• • 
• • •
_
?~~'.oo.
': !;r.. . kO,25
• •....•_•
• ..  .
. 0 _ c){ ]  0  n01
  .    f    .
~

 .•. .
.  .
___ [50%] 0[60%]
 _.    ..         _.  _.
~[80%] 0,2
[100%] 0,15
0,1
0,05
2
3
4
5
alb
Figure 2.3 Kevlar, rectangular plate, all clamped edges, uniform load {(0pl90qhols; p + q =5.
26
2,5
................................. .
• • • • 2
 . _.   _.   _.  _.    
_.
_[50%]
1.5
0[60%] k
+ [80%] ~[100%]
0,5
.......... _ ..... .
2
3
4
5
alb
Figure 2.4. Kevlar, rectangular plate, all supported edges, uniform load {(Opl90qho} s ; p + q
=5
Results for glass fibre composite plates follow the same trends as those observed for carbon and aramid fibres. As might be predicted, values reported for fibreglass are the least stiff of the three systems analysed. The stiffest plate is composed of an unbalanced configuration (100% of fibres in the transverse direction): k
=0.68 and k =3.2 for a plate
with b > 2.5 a, and clamped and simply supported along the four edges, respectively (Fig. 2.5 and 2.6). For a balanced configuration: k = 1.15 and k = 5.7 for a plate with b > 2.5 a, and clamped and simply supported along the four edges, respectively.
27
....
1,2
~
0,8
.
..... . . . .
~.~;.~~..~.~;.~~
~.
/
~
_ _ [50%] 0[60%]
kO,6
+[80%] ~[100%] 0,4
0,2
2
3
5
4
alb
Figure 2,5 Scotchply, rectangular plate, all clamped edges, uniform load {(Opl9Oqhols; p + q =5,
6
_ _ [50%] 0[60%] +[80%] ~[100%]
2
   _ ... _........................  _ ... _. _.
2
4
3
5
alb
Figure 2.6 Scotchply, rectangular plate, all supported edges, uniform load {0pI90qhols; p + q =5,
28
2.3 Homogenisation of laminated plates It has been fotmd through experience and demonstrated analytically that ply groups in a laminate should be dispersed or
spliced as much as possible to improve laminate strength and toughness. In a finely dispersed laminate, all ply groupings have as few plies as possible. If we have a total of 16 plies each of 0° and 90° orientations, the most dispersed symmetric laminate will be [0/90] repeated eight times at the top half of the laminate, and [90/0] eight times at the bottom half, which is shown on the right in the matrix below. The least dispersed laminate will be eight [0] and eight [90] at the top, and eight [90] and eight [0] at the bottom.
The fewer plies in a ply group, the smaller the percentage of this ply group will be in a total laminate. When the ply group fails, the effect is more localised in a dispersed laminate than in a laminate having fewer but thicker ply groups. One way to build up a highly dispersed laminate is to use repeating sublaminates, which is therefore one of the recommended design practices. Let us consider the sublaminate [0/45/45]. By means of the classical laminated theory described in Chapter 1, for one repetition, the normalised stiffness matrix ABBD presents the following configuration (normalised stiffness matrix is not symmetric): 1
[~ ~J=
19.989 6.536 .000
6.536 11.862 .000
.000 .000 6.660
4.019 1.310 1.355
1.310 1.399 1.355
1.355 1.355 1.310
12.058 3.930 4.064
3.930 4.198 4.064
4.064 4.064 3.930
22.669 5.662 2.799
5.662 10.929 2.709
2.709 2.709 5.787
For two repetitions, the normalised stiffness matrix ABBD of the laminate [0/45/45]2 is given by the following expression:
[~ ~J=
19.989 6.536 0.000
6.536 11.862 0.000
0.000 0.000 6.660
2.010 0.655 0.677
0.655 0.700 0.677
0.677 0.677 0.655
6.029 1.965 2.032
1.965 2.099 2.032
2.032 2.032 1.965
20.659 6.317 0.677
6.317 11.628 0.677
0.677 0.677 6.442
The normalised stiffness matrix ABBD of the laminate [0/45/4513 presents the following configuration:
29
19.989 6.536 0.000
6.536 11.862 0.000
0.000 0.000 6.660
1.340 0.437 0.452
0.437 0.466 0.452
0.452 0.452 0.437
4.019 1.310 1.355
1.310 1.399 1.355
1.355 1.355 1.310
20.287 6.439 0.301
6.439 11.758 0.301
0.301 0.301 0.563
[~ ~]= For five repetitions, the normalised stiffness matrix ABBD of the laminate [0/45/45]5 is given by the following expression: 19.989 6.536 0.000
6.536 11.862 0.000
0.000 0.000 6.660
0.804 0.262 0.271
0.262 0.280 0.271
0.271 0.271 0.262
2.412 0.786 0.813
0.786 0.840 0.813
0.813 0.813 0.786
20.097 6.501 0.108
6.501 11.824 0.108
0.108 0.108 6.625
[~ ~]= The normalised stiffness matrix ABBD of the laminate [0/45/45]8 presents the following configuration: 19.989 6.536 0.000
6.536 11.862 0.000
0.000 0.000 6.660
0.502 0.164 0.169
0.164 0.175 0.169
0.169 0.169 0.164
1.507 0.491 0.508
0.491 0.525 0.508
0.508 0.508 0.491
20.031 6.522 0.042
6.522 11.847 0.042
0.042 0.042 6.64
[~ ~]=
For fifteen repetitions, the normalised stiffness matrix ABBD of the laminate [0/45/45115 is given by the following expression: 19.989 6.536 0.000
6.536 11.862 0.000
0.000 0.000 6.660
0.268 0.087 0.090
0.087 0.093 0.090
0.090 0.090 0.087
0.804 0.262 0.271
0.262 0.280 0.271
0.271 0.271 0.262
20.001 6.532 0.012
6.532 11.858 0.012
0.012 0.012 6.656
[~ ~]=
For one sublaminate, since the laminate is nonsymmetric, matrix B is not zero and since the laminate is balanced, this configuration is orthotropic in plane stress but anisotropic in bending. For the laminate [0/45/45] 15 all the elements
30
of matrices B and terms D13 y D23 are lower than 1. Thus, it has been shown that increasing the number of sublaminates, matrices B tend to zero and values Dij tend to Aij. In general, when the number of repetitions is higher than ten, the laminate behaves as a homogeneous material and can be treated as an orthotropic nonlaminated material. 2.4 The freeedge effect When a multidirectional laminate is subjected to tension, compression or bending loads, a delamination process occurs along the free edges of the structure. The resultant interlaminar stresses present significant values along a width approximately equal to the laminate thickness. Delamination along the straight free edge of composite laminates under an inplane uniaxial load has been observed since the early 1970s. Since then a large amount of work has been reported on the freeedge problem in composite laminates, indicating that freeedge delamination is attributed to the existence of interlaminar stresses which are highly localised in the region of a free edge under inplane loading. It has been shown by Kim4 (in Pagano) that in addition to interlaminar tensile stress, other mechanisms such as transverse cracking and interlaminar shearing appear to be significant at the onset and growth of delamination. The [O/901±45]s laminate which has a compressive interlaminar normal stress does not show any delamination under static
tension, but under fatigue tension shows considerable delamination at the interface between the +45° and 45°plies. The interlaminar shear stress at the +45°and 45° interface is not large enough to reach the interlaminar shear strength under static loading, but under fatigue loading, the shear stress becomes significant because of the high fatigue sensitivity of the epoxy matrix. The next section covers several methods for the suppression of delamination by designing proper stacking sequences, reinforcing free edges, and toughening the matrix.
2.4.1 Optimum design/or controlling delamination In most cases the presence and growth of freeedge delamination significantly reduces the loadcarrying capability and stiffness of composite laminates. Because of this adverse effect of delamination on the integrity of composite structures, a great deal of work has been reported in the literature. However, most of this work has been concerned with the aspects of stress analysis and prediction of delamination initiation and growth. Very little work has been reported on the aspect of controlling delamination. Delamination can be alleviated by employing a tough material system and/or a change in laminate configuration. A number of different approaches are considered in the literature, including:
• A design of a proper stacking sequence of a laminate. 4,5,6,7 • Reinforcing the freeedge regions by stitching or wrapping. 8,9, 10 • Using a tough resin or altering the mechanical properties of certain layers in the region of potential delamination by adding or replacing some layers' with toughened materials, such as adhesive film, hybridisation, etc. 11 ,12 It has been shown by Tsai3 that for static loads, a spiral stacking sequence of Qisotropic laminates reduces the
delamination normal stress component considerably, see Fig. 2.7
31
:. Z5, I \
[
2.otl \
.. , .. I
\
\
tS+
I,
\
1511I •., i ~
[45/90/0/45)5.
0
(45
[(0]
0 I
~I'.
20
90]
'6
~
1.6
~
SpiIal StackiDg (prefened)
I
20
[Q/9D(:l45]~+. I ~O'z
Non spiral stacking
40
Figure 2.7 Effect of a spiral stacking sequence on delamjnation normal stress component According to Kim (Pagano)4 for fatigue loads, an apropriate stacking sequence for a given laminate can provide a considerable reduction in the interlaminar stresses. The effect of the interlaminar normal stress in the [+45/0/90]s laminate is intensified considerably with an interchange of the 90° and 0° layer positions. This increase of interlaminar normal stress triggers the delamination at a much lower stress level. Let us consider a Qisotropic laminate of ±30° and 90° plies. The stacking sequence of [±30 190]s generates a tensile interlaminar normal stress at the free edge in the midplane under applied uniaxial tension and, thus, the laminate is delamination prone. If we change the stacking sequence to that of a [90/±30)s laminate, then the freeedge normal stress becomes compressive, which does not cause delamjnation. As another example, let us consider 16 plies of [0/±45/90hs and [02/±452/902]s. The maximum interlaminar normal stress at the midplane is much smaller in the dispersed plies than in the grouped plies. The former dispersed laminate [0/±45/90hs does not display any delamination until final failure under static loading. A ~te design with a proper stacking sequence can reduce the interlaminar tensile stress component in such a way that the probability of delamination will be greatly reduced or eliminated. By means of homogeneous laminates, delamination can be reduced considerably. Free edge stress is inversely proportional to the repeating index r (see Fig. 2.8, Tsai3). The tendency to delamjnate is drastically reduced if many repeated sublaminates are used. The same tendency, i.e. higher r, will make LamRank (a software package by Tsai3 that ranks laminates in terms of inplane strengths) applicable to designing for flexural loads. It is therefore necessary to use sublaminates that are as thin as possible.
32
lozlr)1 lUzl r=1
Lamina'te code
1.0
, . . . .         repeating index C.B O.G
0.4 0.2
2
3
4
5
& 7
8
Figure 2.8 Effect of number of sublaminates on free edge stress. It is possible to prevent or delay the freeedge delamination by suppressing the interlaminar stresses by means of free
edge reinforcement (Kim (Pagano)4). Figure 2.9 shows a specimen reinforced with fibre glass woven cloth using a structural adhesive. the reinforced specimen does not show any evidence of delamination at an applied axial tension of 552 MPa, whereas extensive delamination occurred in the unreinforced specimen subjected to an applied tension of 414 MPa. Delamination in this specimen was initiated at 365 MPa as indicated by acoustic emission. No delamination signature by acoustic emission is observed in the reinforced specimens until final failure. The delamination threshold strain is an average of four specimens and is determined by acoustic emission. The reinforced specimens of the frrst six laminates do not show any delamination until final failure, but the last three laminates, which are subjected to a larger value of crz, all delaminate prior to failure. The strength of the reinforced specimen increased by 140% compared with the unreinforced specimen. The large increase in strength suggested that the effect of delamination on static strength may be much more significant in matrix controlled failure modes than in fibrecontrolled failure modes.
5"
~I 0.125" ~
END TAB
REINFORCEMENT "
T
MATERIAL: FIBER GLASS CLOTH ADHESIVE: EPON 828 Figure 2.9 Minimisation of delamination effect by using a reinforcement.
33
T .75"
Resistance to delamination can also be increased by employing a tough matrix such as thermoplastic. No delamination is observed in the [±30/90]s laminate of PEEK!AS4 graphite composite, but as discussed earlier, this laminate with epoxy resin experiences extensive delamination. However, there will be some sacrifice in performance in other parameters, such as compressive strength and temperature capability. Other research work on the toughening of laminates that are prone to delamination introduce an interleaf or adhesive layer. Chen et aIll performed finite element analysis of the freeedge problem for a specimen containing an adhesive layer at the midplane which is confined to 3.2 mm from the free edge. The adhesive strips reduce the interlaminar stresses and improve the delamination resistance.
Soni and Kiml2 conducted analysis and experiment for a [01±45/90]s laminate containing a structural adhesive layer in the midplane where the critical interlaminar normal stress is present. The stress level at the onset of delamination is increased by approximately 40%. It is conceivable to control freeedge delamination by novel design of stacking sequence in conjunction with the proper reinforcement of toughened interfaces without any significant sacrifice of other important performance parameters of advanced composite materials.
2.5 Conclusions At the beginning of this chapter, stiffness and strength properties of some composite material systems were presented. Also, special configurations like SMC and fabrics were analysed. SMC laminates can be treated as unidirectional Qisotropic configurations. It is important to note that fabric and [0/90] unidirectional laminate give similar results in terms of stiffness and strength parameters (errors lower than 20%). Another conclusion arrived at is that balanced fabric is the optimum configuration for square plates subjected to transverse loads. In those cases, where the plate is rectangular but not square (a :;:. b), balanced fabrics do not give good results. For very narrow plates (b> 2.5 a), the deflection obtained is twice the optimum one: unbalanced fabric. The homogenisation of laminated plates was also analysed. Homogeneous laminates are very interesting in terms of design. When the number of repetitions is higher than 10, the laminate behaves as a homogeneous material and can be treated as an orthotropic nonlaminated material. Finally, the freeedge effect has been analysed from the point of view of design optimisation. The following minimise the freeedge effect
•
A proper stacking sequence of the laminate.
•
Reinforcing the freeedge regions by stitChing or wrapping.
•
Using a tough resin or altering the mechanical properties of certain layers in the region of potential delamination by adding or replacing some layers with toughened materials, such as adhesive film, hybridisation.
References 1347 give further information about the freeedge effect. In the following chapters, shells, plates and sandwich constructions will be analysed.
34
References
1.
Tsai S W, 'Composites Design', Think Composites, Dayton, OH, 1988.
2.
Antequera P, Jimenez L and Miravete A, 'Los Materiales Compuestos de Fibra de Vidrio', Universidad de Zaragoza, 1992.
3.
Tsai S W, 'Theory of Composites Design', Think Composites, Dayton, OH, 1992.
4.
Pagano N J, Composite Materials Series, Volume 5: Interlaminar Response of Composite Materials, Elsevier Science Publishers, Amsterdam, The Netherlands, 1989.
5.
Pagano N J and Pipes R B, The influence of stacking sequence on laminate strength, J Comll Mater 1971, 5, 5057.
6.
Pagano N J, Stress field in composite laminates, Int J Solids and Struct 1978, 14385400.
7.
Lackman L M and Pagano N J, On the prevention of delamination of composite laminates, in: proc structures, structural dynamics and materials conference, Las Vegas, Nevada, April 1974, AIAA Paper 74.
8.
Kim R Y, Prevention of free edge delamination, in: materials and processes  Continuing Innovations, 28th National SAMPE Symposium and Exhibition (1983).
9.
Pipes R B and Daniel I M, Moire analysis of the interlaminar shear edge effect in laminated composites, 1 Compos Mater, 1971, 5, 255.
10. Howard WE, Gossard T Jr and Jones R M, Reinforcement of composite laminate free edges with Ushaped Caps, AIAA 860972 (1986). 11. Chen W S, Rogers C and Aker S, Improvement of edge delamination strength of composite laminates using adhesive layers, ASTMSTP893 (1984) 266285. 12. Soni S R and Kim R Y, Analysis of suppression of free edge delamination by introducing adhesive layer, ICCMVI, eds. F L Matthews, NCR Buskell, J M Hodgkinson and J Morton, Elsevier Science Publishers, London, England, 1987, pp 52195230. 13. Pipes R B and Pagano N J , Interlaminar stresses in composite laminates under uniform axial extension, Comp Mater. 1970, 4.. 538548.
J.
14. Puppo A H and Evensen H A, Interlaminar shear in laminated composites under generalized plane stress, 1 Compos Mater. 1970, 4 204. 15. Whitney J M and Browning C E, 'Freeedge delamination of tensile coupons', J Comp Mater, 1973, 6 300303. 16. Pagano N J and Pipes R B, 'Some observations on the interlaminar strength of composite laminates', InU Mech Sci, 1973, 15,679688. 17. Pagano N J and Soni S R, 'Globallocal laminate variational model', Int J Solids and Struct 19(3) (1983) 207 18. Sendeckyj G P, Maddux G E and Porter E, Damage Documentation in Composite by Stereo Radiography, ASTMSTP775 (1982) 16. 19. Andrews R J, Moran T J and Crane R L, 'New capabilities for ultrasonic imaging of defects in fiber reinforced composites', 11th Ann Mini Symp Aerospace Science and Technology, ed Soni S R, Air Force Institute of Technology, WPAFB, OH, 1985, P 21. 20. Freeman S M, Damage Progression in GraphiteEpoxy by a Deplying Technique, AFWALTR813157 (1981) 21. Kim R Y, private communication.
35
I
22.
Harris A and Orringer 0, Investigation of anglerply delamination specimen for interlaminar strength test, Compos Mater, 1978, 12 285.
23.
O'Brien T K, 'Mixedmode strain energy release rate effects on edge delamination of composites', NASA Technical Report 84592, 1983.
24. Rodini B T Jr and Eisenmann J R, 'An analytical and experimental investigation of edge delamination in composite laminates', in Procceedings of the 4th Conference on Fibrous Composites, eds. EM Lenoe, D W Oplinger and J J Burke. Plenum Press, New York, 1978, pp 441457. 25. Kim R Y and Rosi S R, 'Experimental and analytical studies on the snset of delamination in laminated composites', J Compos Mater, 1984, 18. 26. Wang A S D and Crossman F W, 'Initiation and growth of transverse cracks and edge delamination in composite laminates, Part II, Experimental Correlation', J Compos Mater (supplement), 1980, 14, 71. 27.
Reifsnider K L, Henneke II E G and Stinchcomb W W, Delamination in QIsotropic GraphiteEpoxy Laminates, ASTMSTP617 (1977) 93103.
28. Soni S R and Kim R Y, Delamination of composite laminates stimuled by interlaminar shear, ASTMSTP839 (1986) 2863307. 29. Stalnaker DO and Stinchcomb W W, Load historyedge damage studies in two Qisotropic graphite epoxy laminates, ASTMSTP674 (1979) 620641. 30. Masters J E and Reifsnider K L, An Investigation of Cumulative Damage Development in QIsotropic GraphitelEpoxy Laminates ASTMSTP775 (1982) 40, 31. Rybicki E F and Schmueser D W, 'Effect of stacking sequence and layup angle of free edge stresses around a hole in a laminated plate under tension, J Compos Mater, 1978, 12,300313. 32. Curtis P T , Effect of Edge Stresses on the Failure of
70
..........
..........
C!)
...
z
« en I::I:
C!)
60
jjj
3:
50
~
40
ANGLE
f
Figure 3.5 Weight saving of a fibre glass/epoxy prepreg Scotchply composite dome versus the angle f. For a unidirectional carbon fibre/epoxy laminate ( TIOOIN5208 ) the weight saving of a general spherical dome with respect to A 42 steel is shown in Figure 3.6. The average weight saving can be obtained in terms of the angle fo (Table 3.4).
Table 3.4 Average weight saving for the T3001N5208 fo 15 0 300 45 0 600 75 0 900
AVERAGE WEIGHT SAVING 97.1 % 97.1 % 97.4 % 96.7 % 95.4 % 94.4 %
Thus, in terms of weight saving, the most favourable composite domes are those with fo
=15
0
•
There are very slight
differences between the values obtained for different angles. There is a considerable difference between the average weight saving obtained for this configuration and the other two.
44
100
'0;;/!.
90
T....~......~..
..
~~:::~~!~!~~I
CJ
z 80
:;: cC en
70
tJ:
60
~
w 50
;:
40 o
Ll)
o
Ll)
0
Ll)
0
Ll)
0
Ll)
0
~
~
N
N
M
M
V
V
Ll)
Ll) Ll)
0
Ll)
0
Ll)
0
Ll)
~
~
~
~
~
~
0
m
ANGLEf Figure 3.6 Weight saving of a unidirectional carbon fibre/epoxy resin T300IN520 composite dome versus the angle f. It is interesting to note that the optimum value of the angle fo varies drastically from one material to another. In other
words, a universal optimum angle fo for all composite material systems does not exist. Table 3.5 shows the optimum sublaminate for different values of b and for the four material systems analysed above. The angle b is related to f: f =0° > b =225° f =90° > b =315° The optimum sublaminate is defined for each parallel circle. A fourdigit laminate code for the sublaminate is used. The digits in the code represent the number of plies in the sub laminate, and the order of ply angles selected. The first number represents the number of plies in the sublaminate in the parallel circle direCtion, the second number represents the number of plies in the sublaminate in the meridian circle direction, the third number represents the number of plies at 45° with respect to the parallel circle direction and the fourth number represents the number of plies at 45° with respect to the parallel circle direction. For a generalised rc/4laminate code [4211] means [04"902/45/45].
45
Table 3.5 Representation of optimum sub laminates for four composite materials
8 225 0 2300 235 0 240 0 245 0 250 0 255 0 260 0 265 0 2700 275 0 280 0 285 0 2900 295 0 3000 305 0 3100 315 0
UNIE1200 0055 4600 0433 0433 0622 0622 0100 0100 0100 0100 0100 0100 0811 1900 1900 2800 2800 3700 4600
SCOTCH 5500 0055 0433 0433 0433 0622 0100 0100 0100 0100 0100 2800 4600 5500 6400 7300 7300 8200 8200
TEJE500 0100 0100 0100 0100 0100 0100 0100 0100 0100 0100 0100 0100 0100 0100 0100 0100 0100 0100 0100
T3005208 5500 5500 4600 4600 3700 2800 2800 1900 1900 1900 1900 3700 4600 5500 5500 6400 6400 6400 6400
Once again, it is interesting to note that the optimum sublaminates vary drastically from one material to another. The following conclusions can be drawn: •
Optimum laminate with all the plies in meridian and parallel directions have been selected. Number of plies in meridian and parallel directions are related to the magnitude of Nf and Nl1l inplane loads respectively.
•
Unidirectional material systems analysed here present an optimum weight saving for f
= 51 ° 50', because the
state of stress is unidirectional for this value. This maximum does not appear in the case of a fabric. •
Unidirectional configurations present bad results in a compressioncompression state, with a weight saving of about 45% in the area of f ranged between 0° and 30°. Fabric configurations present better results, with a weight saving of around 67%.
•
The optimum sublaminate for the fabric is [0/90] , i.e. all the fibres are oriented in the meridian and parallel directions.
3.3
Spherical vessel
In this section, a spherical vessel supported on a ring and subjected to the weight of an internal fluid is analysed, the objective being to evaluate in which cases it is worth using composite materials and when this is the case, to assess the weight saving of the composite structure and to obtain the optimum layup for each case. A representation of a spherical dome and the defmition of variables are shown in Fig. 3.7.
46
Figure 3.7 Representation of a spherical vessel and definition of variables. Equations 3.7  3.9 give the inplane loads for the part of the vessel over the support ring (jfo),along the meridian (Nf) and the parallel (Nj1l):
Nf = p.6r2 . (5 + 2·Icosf cos 2f J
[3.11]
fJ
p._ r2. ( I6·cosf =2· cos 2 N¢ = 
6
[3.12]
Icosf
[3.13] According to equations 3.9  3.13, the inplane load Nf suffers a drastic change of value 2 r2_ p / (3 sin2 fo), in the area around the support ring, and the other inplane load Nj1l is decreased in 2 r2  p / (3 sin2 fo).
47
In Fig. 3.8  3.11, inplane load graphics are represented for some values of f o. For all the cases, lines relating Nf and
NjiS are located in the range of ~ (45/90). Moduli of Nf and NjiS are given in MN/m and correspond to
r= 10m
p = 0.01 MN/m3
1
P1·
......
0,9 0,8
.
._._...... ...
••••

0,7 0,6 ..... 0,5 z 0,4 0,3 0,2
~Bl'
° ~1·· •...•. °  
0,1
.....  ....
.... I
I
0,5
1
1,5
N0 Figure 3.8. Representation of inplane loads for fo = 90°.
.........••••• . ..... ..
1
.
0,9 0,8 0,7 0,6
..... z
0,5 0,4 0,3 0,2 0,1 ••••
°°
........... .......... ... ••••• I
I
0,5
1
.
"""', ~
N0
Figure 3.9. Representation of inplane loads for fo = 120°. 48
1,5
......
1
0,5
.......... ..... .......... . 
0
.....
z

I
I
0,5
1
III •• • • •
..... II!I~~k+1
•
1 , 5 ........ ~
2,5
3
.~
0,5
•  1
•
 1 ,5
N0
Figure 3.10. Representation of inplane loads for fo = 150°.
10
0 10
20 3 0
..... z
l .'.
I
'1.
".
'.
20
40
60
80
100
40 50 60 70 80 90 No
Figure 3.11. Representation of inplane loads for fo
=180°.
The relationships between Nf and NjIl shown in Fig. 3.8 to 3.11 depend only upon f, because r and p appear in the factor ( p . r 2 ) in the expressions of both inplane loads Nf and NjIl for angles higher and lower than f o. Therefore, the weight saving is a function of f. In order to find out which material system is efficient in comparison with a standard
49
material (A42 steel), the concept of average weight saving will be used. This parameter is a function of f o' Average weight savings for some composite material systems are represented in Fig. 3.12.
95
~ 0
CJ
z
> c:r:
en
....
::t:
CJ
w
==
90  .   UNIE1200
85 80
__ 111".';
.•, .'
"...,:::,...

...~i .
75
.'
...~~~~
65
     .•
57
I
I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I I
4 CONSTANT THICKNESS PLATES 4.1 Introduction Constant thickness composite plates subjected to buckling and transverse loads (uniform or point load) are most used in engineering applications. In most cases, optimum design is required, the weight being the optimisation criterion and the maximum deflection for transverse loads, and critical compressive force for buckling loads being the parameters to be optimised. Usually, stiffness and not strength is used as the optimisation criterion in plates subjected to transverse loads, since failure is associated with very high deflections. Three studies have been carried out on constant thickness plates subjected to transverse loads: First, three fibre glass composite systems (unidirectional, fabric and chopped strand matting) have been analysed and the influence of several layups on the maximum deflection has been reported for a wide range of aspect ratios. Second, three unidirectional composite systems (carbon, aramid and glass fibres) have been studied and the influence of variation of e in angleply laminates [:te] has been analysed as a function of the aspect ratio. Finally, the influence of rotation of crossply laminates [0190] on the maximum deflection of the plate has been reported as a function of the aspect ratio for the three material systems described above. A buckling study of constant thickness plates has also been carried out. Uni, biaxial and shear loads have been treated for a carbon fibre plate with two boundary conditions: simply supported and clamped along the four sides of the plate. Optimum sublaminates and critical loads are obtained for each case. The behaviour of the optimum angle ply laminates is compared with the isotropic configuration and aluminium, for design optimisation purposes.
4.2 Design optimisation of composite plates in bending A study of maximum deflection of rectangular composite plates is carried out in this section by means of the theory explained in Chapter 1. A simply supported plate subjected to uniform load is analysed (Figure 4.1). Bending and interlaminar shear effects are taken into account. References 123 give several proceedings to optimise composite plates in bending.
a
I
Figure 4.1 A rectangular simply supported plate subjected to a uniform load. Three fibre glass material systems are considered : • UNIDE500 unidirectional fibre glass/polyester system. Vf = 51.85 %. By =10.289 MPa.
59
• FABES80 fabric fibre glass/polyester system. Vf = 40.91 %. Ey =19.817 MPa. •
CSME600A chopped strand matting system. V f = 16.51 %. Ey =7.733 MPa
For a uniform load q, the maximum deflection is given by the following expression: [4.1]
For a central load P, the maximum deflection is: [4.2]
4.2.1 Influence of layup on maximum deflection The maximum deflection of square ( alb = 1 ) simply supported and clamped plates subjected to uniform load does not depend upon the layup, as shown in Fig. 4.2 and 4.3. For rectangular nonsquare plates ( alb > 1), the optimum layup is [90] for simply supported and clamped plates, a substantial difference between the values of k for the optimum layup and for the rest of laminates is reported. For simply supported plates, deflections of laminates [±4S], Qisotropic and [0/90] are very close for aspect ratios ranged between 1 and 2.S. For aspect ratios higher than 2.5 , differences among the deflections of these three laminates increase, the least stiff being [±4S]. For clamped plates, the ranking of laminates in terms of stiffness is [90], [0/90], Qisotropic and [±4S] for all the aspect ratios considered. The values of k are very similar for a square plate ( alb =1 ) for the four layups analysed, as shown in Fig. 4.2 and 4.3:
10
.............................................................. ..
8
k
B
(+45145)
•
Qiso
•
•
2
............................................................. .
o
1
2
4
3
5
6
alb Figure 4.2 Uniform load simply supported plate, UNIDESOO.
60
(0190) (90)
2
............................................................ .
k
a
2
4
3
5
a
(+45/45)
•
Qiso
•
(0/90)
0
(90)
6
alb
Figure 4.3 Uniform load clamped plate. UNIDESOO. When the plate is subjected to a central point load, the maximum deflection of square ( alb = 1 ) simply supported and clamped plates depends upon the layup, the optimum layup being [±4S], as it is shown in Fig. 4.4 and 4.5. For simply supported plates, deflections of laminates [±4S], Qisotropic and [0/90] are very close for aspect ratios ranged between 2.S and S. For clamped plates, all the layups considered show very close deflections for all the aspect ratios analysed.
10
................................... ..
8 6
........................................................... .
a
(0/90)
Qiso
.......................................................... ..
• • o
(90)
k
4 2
........................................................... .
a
2
4
3
5
6
alb
Figure 4.4 Point transverse load, simply supported plate, UNIDESOO.
61
(+45/45)
5
........................................................... ..
4
.........
3
........................................................... ..
2
............................................................ .
~.I... l .. J ... ~.... ~ ........ .
k
o
(+45/45)
• •
Qjso
0
(90)
(0/90)
6
5
4
3
2
B
alb
Figure 4.5 Point transverse load clamped plate. UNIDE500. Behaviour of the FABE580 fibre glass fabric configuration is similar to the unidirectional mentioned above. Substantial differences exist in the values of k. This parameter for the fabric is 2.5 times bigber than the unidirectional configuration, as shown in Fig. 4.6 to 4.9.
30 .............................................................. .
20 ...................................... ..
~~.~.~.~~
.......... ,____________________,
k
10 ............ .
B
(+45/45
•
Qjso
•
(0/90)
. ............................................ L...._ _ _ _ _  '
04~~~T_~T_~~~r~~
o
1
2
4
3
5
6
alb
Figure 4.6 Uniform load, simply supported plate, FABE580.
62
5
4
3 k
.......................................................... ..
2
B
(+45/45)
•
Qiso
......... .................................................... L _•_ _ _ (0/90) _ _..J
O~~~~~~~~~~~~~
o
2
4
3
5
6
alb
Figure 4.7 Uniform load, clamped plate, FABE580.
30 ....................................................... ..
20 ........
~ ..~....~... ~....~ ... ~....~ ....... .
k
10 ........................................................ .
o
2
1
4
3
B
(0/90)
• •
Qiso (+45/45)
6
5
alb Figure 4.8 Point transverse load, simply supported plate, FABE580.
15 .......................................................... .
10 .........
~~~I~I~I ........
k
B
(+45/45)
•
Qiso
•
(0/90)
5 ......................................................... ..
o
2
4
3
5
6
alb Figure 4.9 Point transverse load, clamped plate, FABE580.
63
Deflections of chopped strand matting plates subjected to uniform and central load are strongly dependent on the boundary conditions, as shown in Fig. 4.10 and 4.11. For simply supported plates, the stiffness increases substantially for aspect ratios close to 1. Except for the case of a square plate, the deflection of clamped plates does not depend upon the aspect ratio. 15 ........................................................ .
10 ....................................................... . 181
k
~.t
Clamped Simply
supported
5 ....................................................... .
04~~~~~~~~~r~~~~
o
3
2
4
6
5
alb Figure 4.10 Uniform load, CSME600A.
. . . . r..:. .~. .~. ~. .:. .~. . . . .
20 ........................................................ .
181
k
10
Clampled
~.t Simply B
B
B
B
B
B
supported
EI
O;~~~~~r~~~~~~~
o
1
2
4
3
5
6
alb Figure 4.11 Point transverse load, CSME600A.
4.2.2 Maximum deflection of the sublaminate [±6] The maximum deflection is strongly dependent on the variation of e on angleply laminates, as shown in Fig. 4.12 to
4.17. The stiffest laminate is [90] and the least stiff is [0] for all the aspect ratios considered. Small differences of values of k are reported in ;the ranges [0] to [±15] and [±60] and [90]. Carbon, aramid and glass fibre composite laminates show similar values of k for the layup [90] and high aspect ratios. For low values of the aspect ratio, deflections for the glass fibre system become the highest and for the carbon fibre system the 10wesL
64
3,5
3
2.5
. . . . ......
............... _.........  _.
                    
I • 10
I
2
(0)
[+15/15) :
  +   [+30/30)

k 1.5
[+45/451
,*,. [+60/601
.
.~.'~'~.
I'cA [+75/75)
".(90)
0.5
• • • • • 2
3
4
5
alb
Figure 4.12 TIOO/5208, rectangular plate, all clamped edges, uniform load, {[+9/ 9] 1o} s.
16
14
12
    (0)
c:
/
10
•
[+15/15)
    [+30/30) ~ [+45/·45)
k 8
•
..... ·i··~
6
[+60/60)
I'cA [+75/75)
".(90) 4
2
2
4
3
5
alb
Figure 4.13 1'20015208, rectangular plate, all supported edges, uniform load, {[+9/911 0 }s.
65
3,5
..
..
3 
2,5
(0)
= (+15/15) 2
(+30/30)
k
~
1,5
• 
..

(+45/·45)
.*t
(+60/60)
fr (+75/75)
< CIS
E
0,002 0,001
90 kg/m3
 :~ •+~
°°
+
.+
+.
0,01 0,02 0,03 0,04 0,05 0,06 0,07 0,08 0,09
+
0,1
core thickness (m) Figure 5.21 Maximum deflection versus core thickness for some core foams. Carbon fibre and aluminium honeycomb core.
99
sandwich SCOTCHPLVPUR 0,05

0,04
c o oG)


0,03
>< CIS E
0,02
 30 kg/m3
G)
[J
"C
60 kg/m3
• 90 kg/m3
0,01
°°
0,01
0,02 0,03 0,04 0,05 0,06 0,07 0,08 0,09
0,1
core thickness (m) Figure 5. 22 Maximum deflection versus core thickness for some core foams. Glass fibre and polyurethane foam core.
sandwich T300INS208Honeycomb 90
G)
::s CIS
>
•
IX:
80
~.
70
~~~

60
~.
50
~~
40 30
/
~~ • :~ ~~
20 10
 30 kg/m3 60 kg/m3
• 90 kg/m3
. =
~ ~~~...
...~ ...
°°
[J
A
...

0,01
0,02
0,03
0,04
0,05
0,06
0,07
0,08
0,09
0,1
core thickness (m) Figure 5. 23 Rvalue versus core thickness for some core foams. Carbon fibre and aluminium honeycomb core.
100
sandWich SCOTCHPLVPUR 50 45
~+
40
~~
35 Q)
30
as
:::J
25
>I
a:
20 15
~~~:
~~
[] 60 kg/m3
~~ ~~.~ ~!~~~/ +
10 5
 30 kg/m3
+
90 kg/m3

...
/~.~.+
°°
0,01
0,02
0,03
0,04
0,05
0,06
0,07
0,08
0,09
0,1
core thickness (m) Figure 5.24 Rvalue versus core thickness for some core foams. Glass fibre and polyurethane foam core.
sandwich T300/N5208Honeycomb 14 12
~~
/+
C)
.:.:: J:
C)
10 8
~~.,/+ +
6
CI)
==
~~.,/+
4
~~ ~! /. + ~ +:.~


 30 kg/m3 [] 60 kg/m3 +
90 kg/m3
2
°°
0,01
0,02
0,03
0,04
0,05
0,06 0,07
0,08
0,09
0,1
core thickness (m) Figure 5.25 Weight versus core thickness for some core foams. Carbon fibre and aluminium honeycomb core. 101
sandwich SCOTCHPLYPUR 14
~+
12
/+
~~
10

/"+
• 30 kg/m3
+
C)
.:.::
~
8
/"+ ______________ .+L . ___• +
.c
6
C)
CD
~
.,;'
;:
~+
.
I
_ _•
.  •
.
.
[] 60 kg/m3 +
90 kg/m3
+.,;'~~.~
4 2
°°
0,01
0,02 0,03 0,04 0,05 0,06 0,07 0,08 0,09
0,1
core thickness em) Figure 5. 26 Weight versus core thickness for some core foams. Glass fibre and polyurethane foam core. As shown in Fig. 5.27, the weight of the structure decreases dramatically in a certain range of core thickness (90150 mm). If the core thickness is increased from the upper limit of this range ( thickness higher than 150 mm), the weight of the structure decreases very slowly. Therefore, in terms of weight saving, there is a range (90150 mm) where increasing the core thickness is a very efficient design possibility, but in the range of core thicknesses higher than 150 mm, other designs, such as implementing reinforcements in the sandwich, must be considered.
80
\~
70

60
CD
40
     _.\                     •.. 
. c 50 C)
==
If "If
.....
~".11
           ..............••••••••••••••••••••••••            
30 20 10
°
°
100
200
300
400
Thickness
Figure 5.27 Weight (kglm) versus core thickness. Glass fibre and polyurethane foam core 2 m width with uniform load (to MPa) 102
Although Fig. 5.27 demonstrates a design curve for a particular sandwich geometry and fibre/resin type, many such curves can be derived from a knowledge of the sandwich behaviour of different geometries and fibre/resin types as a function of the sandwich thickness.
5.3.4 Optimum design of reinforced sandwich constructions Simple reinforcements are especially efficient for those applications where there is a unidirectional stress, for instance in narrow simply supported plates subjected to uniform loads (Fig. 5.28 and 5.29). For square plates, there are stresses in the transverse and longitudinal directions, and therefore reinforcement should be used in both directions. Great difficulties can be encountered when joining perpendicular reinforcements.
Figure 5.28 The structure.
Figure 5.29 The sandwich and reinforcement.
Weight is the optimisation criterion and the maximum deflection should not be higher than the ratios span/250 or span/500 for fibreglass and carbon fibre skins, respectively. This is a rule used in engineering applications design to take account of stiffness and strength of the sandwich structure.
Skin thickness, reinforcement thickness, foam density and number of reinforcements per unit width have been optimised. For carbon fibre skins and aluminium honeycomb, with a 2.5 m span and a 30 MPa load, the reinforced design is considerably better than the nonreinforced one for sandwich thicknesses between 110 and 280 mm (Fig. 5.30). For thicknesses between 80 and 110 mm, one solution exists for reinforced sandwiches but it is not possible to meet 103
the requirements with nonreinforced sandwiches. For thicknesses greater than 280 mm, results from reinforced and nonreinforced sandwiches are similar (the weight saving is 22%). The optimum number of reinforcements is three per metre in all cases. Thus, the efficiency of the implementation of reinforcements depends on the sandwich thickness.
120
_.
100 80

60
CD
40
.c
_. 
••
11 
. 
rr. rr. rrr; rr;









  .   Non reinforced
.rr.r·G•
·Ii...........
C)
3:
,••   _.             .     _...............    
~
Reinforced
20 0 100
0
200
300
400
Thickness Figure 5.30 Carbon aluminium honeycomb. Weight (kglm) versus thickness for a sandwich 2.5 m width with uniform load (30 MPa).
Similar graphics are obtained by varying the load magnitude, span and the material system. Results are shown in the table below:
Table 5.1 Optimisation of reinforced sandwich constructions
Facing
Core
material
material (m)
Span
Load
Minimum
(MPa) thickness for reinforced
Minimum
Minimum
Minimum
thickness
weight
weight
for nonreinforced
for reinforced
for nonreinforced
sandwich (mm) sandwich (mm)
sandwich (Kglm) sandwich (Kglm)
Carboni
Alum.
2.5
30
78
122
28
36
WS: 22%
epoxy
honey
2.5
50
100
183
35
51
WS: 31%
comb
2.5
70
124
241
42
74
WS: 43%
30klm3 2
30
73
100
18
22
WS: 18%
2
50
78
144
23
32
WS: 28%
2
70
100
186
27
40
WS: 32%
1.5
30
40
75
10
13
WS: 23%
1.5
50
54
100
13
18
WS: 28%
1.5
70
70
133
15
23
WS: 35%
1
30
30
50
4
6
WS: 33%
1
50
32
68
6
8
WS: 25%
1
70
34
95
7
10
WS: 30%
104
Facing
Core
Span
material
material (m)
Load
Minimum
(MPa) thickness for reinforced
Minimum
Minimum
Minimum
thickness
weight
weight
for nonreinforced
for reinforced
for nonreinforced
sandwich (mm) sandwich (mm)
sandwich (Kglm) sandwich (Kg/m)
Eglass
PUR
2.5
10
55
105
30
40
WS: 25%
polyester
30Klm3 2.5
30
100
248
43
90
WS:48%
2.5
50
120
380
55
140
WS: 61%
2
10
50
83
18
25
WS: 28%
2
30
68
200
28
62
WS: 55%
2
50
88
300
36
95
WS: 62%
1.5
10
53
63
10
14
WS: 28%
1.5
30
63
145
18
34
WS:47%
1.5
50
70
215
20
50
WS: 60%
1
10
34
40
5
6
WS:8%
1
30
36
100
7
14
WS: 50%
1
50
38
140
10
22
WS: 55%
It has been shown that the weight saving obtained by using reinforced sandwiches is strongly dependent on the load.
The higher the load, the higher the weight saving. Variations of weight saving with the span of the plate are not significant.
5.4 Buckling 5.4.1 General buckling A sandwich beam subjected to compression may fail because of a condition of instability that involves the whole beam. For this reason it is called 'general buckling' (Fig. 5.31 (a».
105
\
TTTT b)
a)
!!!!
!!!!
(
r
~
It ~
TTTT
TTTT
c)
d)
Figure 5.31 Sandwich failures due to a buckling load: (a) general buckling; (b) crimping; (c) wrinkling; (d) dimpling. General buckling may also occur when the stress in the facings and in the core is lower then the allowable stress. The load that determines sandwich instability depends on such parameters as the beam inplane size and the constraint conditions, which can only be partially modified at the design stage. Other quantities, which are equally important for the defmition of buckling load, depend directly on the type of sandwich. They are: • Flexural rigidity of the sandwich. • Thickness of the facings . • Elastic properties of the facings. • Core thickness . • Shear modulus of the core. To avoid this type of failure, it is necessary to ensure that the general buckling load is higher, according to a suitable factor of safety, than the predicted compression stress. When choosing the safety factor one must take into account that the theoretical formulae used to predict the general buckling critical load are less reliable than those for the calculation of sandwich stresses. If general buckling is feared, one may:
• Use facings with a higher elastic modulus material. • Increase facings thickness. 106
• Increase core thickness. • Use a core material with higher shear modulus. F
1
F
1
F
F
1
1
lcr= 0.7071
lcr= 0.5 1
Figure 5.32 General buckling of a sandwich structure and critical lengths of some boundary conditions.
In the case of a sandwich with a relatively low length/thickness ratio and where shear rigidity is small in comparison with flexural rigidity, sandwich general buckling will assume a typical configuration, (Fig. 5.54 (b». This failure mode, typical of sandwich structures, is called 'shear crimping'. The total load per unit length capable of producing crimping is practically independent of facing properties. On the other hand, it increases linearly with the following parameters: • Core thickness. • Shear modulus of the core. To increase the total critical crimping load, one should: • Increase core thickness. • Use a higher shear modulus for the core. 5.4.1.1 General buckling of a sandwich beam It has been shown by Tetil that the critical stress causing the general buckling of a sandwich beam under compressive load (Fig. 5.55) is given by:
1
[5.1]
O"cr b = where:
[5.2]
107
and <Jer b
=
critical buckling stress (N/mm 2)
El
=
sandwich flexural rigidity (N/mm2)
b
=
beam width (mm)
SFl,2
=
thickness of facings 1,2 (mm)
ler
=
free length of the sandwich beam (mm)
GA
=
sandwich shear rigidity (N)
It is easily verified that, when l~r GA« El, equation 5.1 reduces to: GASA
[5.3]
<Jcrb=   
SFt In this case a particular mode of general buckling occurs, usually called 'shear crimping' (Fig. 5.54 (b». Considering that the quantity <Jcr b SFt represents the total Crimping load per unit width of the sandwich, it can be concluded from equation 5.3 that this load is only dependent on the shear rigidity GA. 5.4.1.2 General buckling of a rectangular plate compressively loaded along two opposite edges The critical stress causing the general buckling of an isotropic rectangular sandwich plate with equal facings and isotropic core, subjected to a compressive load along two opposite edges, is given by the following equation: EF
[5.4]
2
4
1VF
where: [5.5]
and <Jer p
=
critical buckling stress (N/mm 2)
K
=
buckling factor, to be evaluated from Fig. 5.56 and 5.57
EF
=
facing compression modulus (N/mm2)
vF
=
facing Poisson's ratio
b
=
length of the plate loaded edge (mm)
SA
=
distance between the facings centroids (mm)
SA
=
core thickness (mm)
SF
=
facing thickness (mm)
It is easily seen, from the graphs in Fig. 5.56 and 5.57, that the socalled 'shear deformation factor', S, must be evaluated in order to define the buckling factor K o.
1z
°Smax 1
o
2 z
o 1
Figure 6.4 Distribution of 0"5 for a twosides tapered plate and aM/ax > o.
121
t
In Fig. 6.56.7, the distributions of al
,a3 and a5 through the thickness for unidimensional oneside tapered plates and
linear bending moment distributions with
aM/ax> 0 are shown. Obviously, to taper the plate on just one side leads to
nonsymmetrical distribution with peaks of interlaminar stresses near the surface which is tapered.
o 2z
o 1 Figure 6.5 Distribution of al for a oneside tapered plate and aM/ax> o.
x
+
(J3max
1
o 2z
o 1 Figure 6.6 Distribution of a3 for a oneside tapered plate and aM/ax> o.
122
t
t
L:d Tz
x
I
~
0'5 O'sm.ax 1
0
2z 0
t
Figure 6.7 Distribution of 0"5 for a oneside tapered plate and aM/ax> o. Figures 6.86.10 show the distributions of 0"1 ,0"3 and 0"5 through unidimensional twosides tapered plates and linear bending moment distributions with
aM/ax < o. It is apparent that the sign of aM/ax
has a strong influence on the
distributions of longitudinal and interlaminar stresses.
0'1m.ax 1
0
2 z o 1 Figure 6.8 Distribution of 0"1 for a twosides tapered plate and aM/ax < o.
123
t
Tz
2z t o
1 Figure 6.9 Distribution of <J3 for a twosides tapered plate and
aM/ax < o.
~ Tz
x
I
+
O's O'Smax
0
2 z
o
t
1 Figure 6.10 Distribution of <J5 for a twosides tapered plate and
aM/ax < o.
Finally, Fig. 6.11 to 6.13 represent the distributions of <Jt ,<J3 and <J5 through unidimensional oneside tapered plates and linear bending moment distributions with
aM/ax < o. 124
1z
2z
o 1
Figure 6.11 Distribution of 01 for a oneside tapered plate and aM/dx < o.
1z
o 2 z o t 1
Figure 6.12 Distribution of 03 for a oneside tapered plate and aM/dx
o.
t
1
x
(l~DI MP
6 ,~ 5
= 90 • 9 = 15 I::J
4
9
3
2
1
o 2z t
Figure 6.18 Distribution of cr3 for a oneside tapered plate, tl/t=0.2, MIPt=5 and aM/ax> O.
128
5~~
4
I:l
0=
90
•
0=
15
3
2
o 2z t Figure 6.19 Distribution of 0'5 for a oneside tapered plate, tl/t=O.2, MlPt=5 and aM/ax> O. Distributions of 0'1 ,0'3 and 0'5 for tl/t=O.l, MlPt=5 and aM/ax < 0 are presented in Fig. 6.206.22, respectively. Numerical values keep decreasing because of the value of tl/t=O.l. Also, the effect of the angle of variation of thickness can be seen by comparing the distributions for 0=90° and 0=15°.
,. z t
1
x
(lID MP
I:l
4 
•
=90 0 = 15
0
4 
1
2z t
Figure 6.20 Distribution of 0'1 for a oneside tapered plate, tl/t=O.l, MIPt=5 and aM/ax> O.
129
3 ,,
2
M 0"3
III
0
•
0
= 90 = 15
p2 1
o
I
o
1
z
2
t Figure 6.21 Distribution of a3 for a oneside tapered plate, t1/t=O.I, M!Pt=5 and aM/ax> o.
. z t
1
.
x
(lID MP
4 ~~ 3
III
0
• 0
t O"s
= 90 = 15
2
p •1
o 2z t Figure 6.22 Distribution of a5 for a oneside tapered plate, t1/t=O.I, M!Pt=5 and aM/ax> o. The following conclusions can be drawn after analysing the results described above: •
The examination of Fig. 6.26.13 leads to the conclusion that the variablethickness effect presents a strong influence on the distributions of longitudinal and interlaminar stresses. High peaks of interlaminar stresses appear near the areas of change of thickness.
• It is also noticeable by comparison of Fig. 6.26.4 and Fig. 6.56.7, that the distributions of the throughthickness stresses vary as a function of the sign of aM/ax. 130
•
Stress distributions are strongly dependent on tit!, the thickness ratio, as the comparison between Fig. 6.146.16,6.176.19 and 6.206.22, reflect.
•
0,
the angle of variation of thickness has a remarkable influence on interlaminar stress distributions through
the laminate thickness. This can be seen in Fig. 6.146.22. Focusing on optimisation of laminated composite plates, the last four parameters in the above list will be input data, and the optimisation procedure will determine the other parameters on the list except for the angle of variation of thickness. Therefore, the study of this parameter becomes more and more important since the angle of variation of thickness is critical for the mechanical behaviour of variable thickness plates. 6.2.3 Failure mechanisms A variable thickness unidimensional laminated composite plate exhibits a variety of failure mechanisms when subjected to transverse loads. Knowledge of these modes is very important to understand what happens inside the laminate. Once we know the critical failure mechanisms, we will be able to identify the strain components associated with them. Different types of laminated composite plates were tested in fatigue and static conditions: • AS4/35016 graphite/epoxy was used for this work. • The types of testing performed were three point static and dynamic bending. • The load rate for the static testing was 0.06 inlmin (0.001524 mlmin). • For fatigue testing, the frequency was 5 cycles/second, and the load was 60 % of the static failure load. The vertical displacement was controlled. Figure 6.23 shows the threepoint bending testing.
131
Figure 6.23 Three point bending test. After studying the results, the following failure mechanisms have been reported: 1 Delamination. This is the most usual failure mode when the angle of variation of thickness is high. It is due to the fact that a sharp thickness variation generates a peak of interlaminar shear stress near the areas of change of thickness. In Fig. 6.24, a delamination failure in a tapered surface is shown. This mechanism can also be detected in thick plates, though the angle of variation of thickness is low. A representation of this failure mechanism is shown in Fig. 6.25.
Figure 6.24 Delamination failure in the midplane.
Figure 6.25 Delamination failure in the tapered surface. 132
2 Bending modes (compression). This mechanism occurs when the plate is very thin, the variable thickness effect is negligible, and the compression strength is lower than the tension strength in the fibre direction. The following inplane compression failure modes can be distinguished: (a)
Induced transverse tensile failure. Unidirectional composites can fracture along the fibres when loaded by compression by a transverse tensile failure mode, because of the weakness of the matrix and the fibrematrix interface, compared with the strength of the fibres.
(b)
Compressive delamination failure. If a fibre buckles, the fibrematrix interface may fracture in shear and lead to ultimate failure.
(c)
Euler failure. If the matrix is ductile and the interface is strong, the fibre can bend without matrix failure and eventually fracture in bending.
(d)
Microbuckling. A more likely failure mode of unidirectional composite laminates associated with fibre microbuckling and fibre kinking, is shear crippling. Macroscopically, shear crippling looks like a shear failure on a plane at an angle to the direction of loading. Microscopic inspection, however, indicates that shear crippling is frequently the result of kinkband formation.
(e)
Strength failure. The final failure mode exhibited in unidirectional composites is associated with pure compression failure of the fibres. In this case, the fracture surface is likely to be at an angle to the loading direction, usually about 45 0 .
3 Bending modes (tension). This mechanism occurs when the plate is very thin, the variable thickness effect is negligible, and the compression strength is higher than the tension strength in the fibre direction. The following inplane tension failure modes can be distinguished: (a)
Unidirectional composite subjected to longitudinal tensile load. Brittle failure. In this mode, stress concentrations created at the broken fibre ends lead to specimen separation at a, given cross section.
(b)
Unidirectional composite subjected to longitudinal tensile load. Brittle failure with fibre pullout. Variations in bond strength and local load transfer mechanisms from matrix to fibre can lead to the pullout of the fibres from the matrix at fracture.
(c)
Unidirectional composite subjected to longitudinal tensile load. Brittle failure with debonding and/or matrix failure. Finally, in other cases, cracks at different cross sections of the laminate may join together at fracture through fibrematrix debonding or by shear failure of the matrix. This interfibre matrix shear failure and fibrematrix debonding can occur either independently or in combination; i.e., portions of the failure path may exhibit debonding, while matrix shear failure is evident in other regions.
4
Mixed modes. A mixed failure mechanism has been detected in the regions close to the application of the load. 133
There exists a compressive delamination failure due to the bending mode (compression), and crushing due to a compressive peeling or interlaminar normal stress. This mechanism was observed in threepoint bending fatigue testing, after 50 000 cycles. In Fig. 6.26, a representation of this mixed mode is shown.This mixed mode does not appear in the four point bending testing and it can also be avoided by placing a hard rubber pad (6080 durometer) between the load point and the specimen (Fig. 6.27).
Figure 6.26 A mixed compressioninterlaminar normal failure mode.
Figure 6.27 A 3P test bending with a hard rubber pad between the load point and the specimen.
Mter analysing the failure mechanisms described above, the following conclusions can be drawn: •
The critical failure modes are related to two strain components: c 1 or longitudinal normal strain and c5 or interlaminar shear strain.
•
The bending (compression or tension) modes are likely to occur when the plate is thin and the variable thickness effect is negligible. 134
•
The delamination mechanisms are usual in cases where the variable thickness effect is critical (sharp change of thickness). The failure appears in the tapered surface. This mechanism also occurs when the plate is thick, even if the variable thickness is negligible. In this case, the failure appears near the middle plane of the laminate.
•
The mode related to interlaminar normal strains (mixed modes) are due to stress concentrations in the areas near the application of the load. This mechanism can be easily avoided by means of the solutions mentioned above.
6.3
Conclusions
A study on variable thickness composite structures has been carried out This chapter focused on the distribution of stresses through the laminate thickness and failure modes. The following conclusions have been obtained: • The variable thickness effect has a remarkable influence on the behaviour of a tapered laminated composite plate. The distributions of throughthickness stresses are very sensitive to the thickness ratio (tltl) and the angle of variation of thickness. In particular, the interlaminar shear stress reaches very high values in the areas of change of thickness. The peak value can be controlled by modifying some parameters: thickness ratio, angle of variation of thickness, type of loading, etc. The distributions of interlaminar stresses vary with the sign of the bending moment • The failure mechanisms reported in variablethickness composite plates can be grouped in three general
modes: Interlaminar shear mode: This is due to interlaminar shear stresses, and appears in the tapered surfaces when the change of thickness is sharp (high angles of variation of thickness) . It can also appear in the midplane, in thick plates .
• •
Bending modes: These are due to bending stresses. These modes are usual in thin plates, very low angles of variation of thickness and low thickness ratios. They are the typical failure modes in thin, untapered plates. Mixed modes: A compressioninterlaminar normal mode has been found in the area of application of the load in the fatigue testing. This mode does not appear in the fourpoint bending test.
References 913 analyse aspects related to failure of these types of structures. The following chapters will be devoted to the optimisation of variable thickness beams, plates and sandwich constructions.
References
1. Foye R, 'MYanced
Desi~n
Concepts for AdYanced Composite Frames' ,Volume III Air Force Materials 135
Laboratory, Wright Patterson Air Force Base, Ohio, AFMLTR6891, 1968. 2. Waddoups ME, 'Structural Airframe Application of AdYanced Composite MaterialsAnalytical Methods' . Volume IV Air Force Materials Laboratory, Wright Patterson Air Force Base, Ohio, AFMLTR69101, 1969. 3. Waddoups ME, McCullers LA, Olsen FO. and Ashton JE ," Structural synthesis of anisotropic plates ", Presented at AIANASME 11th Structures, Structural Dynamics and Material Conference, Denver, Colorado, 1970. 4. Schmit, LA, " Structural Design by Systematic Synthesis", Proceedings of 2nd National Conference on Electrical Computation, Structure Division, ASCE ,pp. 105, 1960. 5. Schmit LA, Kicher TP and Morrow WM., 'Structural synthesis capability for integrally stiffened waffle plates', AIAA Journal, 1963, 1,282036. 6. Kicher TP, 'Structural synthesis of integrally stiffened cylinders', Journal of Spacecraft and Rockets, 1968,5, 628. 7. Schmit LA., Morrow WM., and Kicher TP, "Structural Synthesis Capability for Integrally Stiffened Cylindrical Shell Shells", AIAA Paper 68327, Palm Springs, California, 1968. 8. Tsai SW and Hahn HT, 'Introduction to Composite Materials', Technomic, Westport Com., 1980, pp. 457. 9. Tsai SW and Wu EM, 'A general theory of strength for anisotropic materials', J. Composite Mat, 1971,5, 58. 10. Roy AK and Tsai SW, '3D Effective moduli of laminated orthotropic plates', to appear in Journal of Applied Mechanics. 11. Ashton JE, 'Analysis of anisotropic plates II', J COI:IijX)site Mat., 1969, 3,470. 12. Miravete A, 'Analisis del Comportamiento Resistente de Laminados de Poliester Reforzado y su Aplicaci6n a los Medios de TranspOrte', Ph D University of zaragoza, Spain, 1984. 13. Miravete A, 'Caracterisation et mise au Point d'un Element Fini de Grande Precision Applicable a des Lamines de Polyester Renforce avec Fibres de Verre', Composites. 1986,4, 20.
136
7 VARIABLE THICKNESS BEAMS 7.1 Introduction In this chapter, a study of optimisation of variable thickness laminated composite beams subjected to transverse loads is carried out. Generally speaking, a beam subjected to a transverse load presents a level of stress which varies substantially from one cross section to another. Therefore, the variation of thickness represents a possibility for reducing the weight of the structure by adapting the thickness of the section to the stress level. There are many applications where this philosophy has been successfully applied. For instance, the weight of the nonsuspended part (suspension system) is critical for the stability of a vehicle. The stability of the vehicle increases by lightening the suspension system. There are several possibilities to tailor a beam in order to optimise the design (Fig. 7.1). The best design consists of a constant width and variable thickness beam composed of a noncontinuous fibre internal part and continous fibre laminates at the external part. If the external part is nonfibre continuous, delamination takes place at a very low stress level. If the crosssection is constant, (width and thickness variable) delamination also takes place.
p
(1
,....'7...
~~~=#
OPTIMUM
~14L~.1
DELAMINATION
PLl4
DELAMINATION
14
L
_I
HEAVY
DIAGRAM OF BENDING MOMENT
Figure 7.1 Scheme of variable thickness composite beams. This chapter is divided into two parts. The first part deals with the behaviour of variable thickness composite beams. An experimental analysis of three types of beams is described and the results of a correlation study between the model
defined in Chapter 6 and this experimental analysis will be shown. The second part of this chapter is devoted to the optimisation of variable thickness composite beams. Solutions for different types of beams, loads and boundary conditions are given.
137
7.2. Behaviour of variable thickness composite beams An experimental study has been carried out in order to assess the accuracy of the theoretical model, as well as to fmd out the influence of the angle of variation of thickness on the strength of a composite plate. •
AS4/35016 graphite/epoxy was used for this work.
•
The type of testing performed was three point static bending.
•
The load rate was 0.06 inlmin (0.001524 mlmin).
•
Three types of specimens were tested. Maximum, minimum thickness and span were the same for the three specimens. The only variable parameter was the angle of variation of thickness: • Specimen OLCP_7001. Angle of variation of thickness: 6°. • Specimen OLCP_7002. Angle of variation of thickness: 45°. • Specimen OLCP_7003. Angle of variation ofthickness: 90°.
•
The span was 8 in (0.2032 metres).
•
The maximum thickness was at the centre of the beam: 0.66 in (0.0167 metres).
•
The minimum thickness was at the end of the beam: 0.28 in (0.007 metres).
•
Longitudinal and interlaminar strains were measured by using strain gauges. The situation of the gauges is reported in Table 7.1. The choice of the points was carried out as a function of the theoretical analysis. Strain gauges were placed at those points whose strain value was critical, according to the results from the finite element method applied to variable thickness laminated composite plates.
138
Table 7.1 Coordinates x and y of strain gauges. Values are expressed in inches (metres)
X
POINT
Y
1
0.0
(0.0000)
0.100
(0.00254)
2
0.0
(0.0000)
0.200
(0.00508)
3
1.0
(0.0254)
0.350
(0.00889)
4
2.0
(0.0508)
0.415
(0.01054)
5
3.0
(0.0762)
0.600
(0.01524)
6
4.0
(0.1016)
0.510
(0.01295)
7
4.0
(0.1016)
0.350
(0.00889)
8
4.0
(0.1016)
0.000
(0.00000)
According to the results of the study on failure mechanisms, critical strain components are the longitudinal strain £1 and the interlaminar shear strain £5. Therefore, both components are analysed for the three types of specimens described above. The scheme of the specimen OLCP_7001 is shown in Fig. 7.2. This specimen was made by tapering the inner part of the plate (Fig. 7.4). The angle of change of thickness is 6°. The failure load was 4950 lb (22 OOON). The upper surface does not pre~ent any failure, in spite of being tapered. Instead of that, a crack appears near the middle plane at the end of the plate where interlaminar shear strains are maximum. The reason for this is that the angle of variation of thickness is very low. A scheme of the situation of the gauges is depicted in Fig. 7.3. The numerical results of the specimen OLCP_7001 are presented in Tables 7.27.4. Tables 7.2 and 7.3 show longitudinal and interlaminar shear strains in the critical points for the failure load, respectively. The maximum value is registered in point number 1 (£5=0.0131).
139
0.66(0.0167)
I 1 (0.025) 14
.1 .1
Figure 7.2 Scheme and measurements of specimen OLCP_7001 in inches (metres).
z
T ~~
3 x
5
4
x
x
lP x x ~E
6 7
~
8
Figure 7.3 Representation of specimen OLCP_7001 and position of gauges.
Table 7.2 Longitudinal strains in specimen OLCP_7001. Load: 4950 Ib (22 000 N).
POINT
8
£1
if
£1
lE3
if
lE3
TESTING
THEORY
8.9
8.6
140
X
Table 7.3 Interlaminar shear strains in specimen OLCP_7001. Load: 4950 lb (22 000 N).
(5
POINT
.
.
(5
lE3
THEORY
TESTING
12_5
13.1 (FAILURE)
1
lE3
2
9.0
8_1
3
6_3
7_3
4
5_7
6_7
5
4_2
5_8
6
3_7
3_1
7
12_7
12_1
The maximum vertical displacement is reported in Table 7.4. In both fields, strains and displacements, an excellent agreement is found between the data and the prediction. Table 7.4 Maximum vertical displacement in specimen OLCP_7001. Load: 4950 lb (22 000 N).
POINT
dZ
8
 0_173
d
TESTING
Z
THEORY
• (0_00439)
 0_161
(0_00409)
The scheme of specimen OLCP_7002 is shown in Fig. 7.5. The angle of change of thickness is 45°. Six steps were designed along the specimen. The failure load was 2960lb (13 150 N). Owing to the fact that the angle of variation of thickness is high, failure appears at the upper surface in the thinnest area of change of thickness. Failure mechanism is a kind of interlaminar shear mode. As theoretical results predict, there is a peak of interlaminar shear strains in the places where the thickness changes. The position of the gauges is shown in Fig. 7.6. The numerical results of the specimen OLCP_7002 are presented in Tables 7.57.7 . Tables 7.5 and 7.6 show longitudinal and interlaminar shear strains in the critical points for the failure load, respectively. The maximum value is registered in point number 3 (£5=0.0131).
141
0_66(0_0167)
0_55(0_014) 0_28(0_007)
I
I
/
I
I
/
/
,
I
2_4(0_061 )
0_41 (0_0 1 0)
'"I .1
6_4(0_162)
I.
.1
8(0_203)
I
1
·1
4_4(0_ 111)
I
\.
.1
Figure 7.4 Scheme and measurements of specimen OLCP_7002 in inches (metres).
lP
z
1 11:
4
3 s(
5 /x
,
/x x
\..
7
\.
)(
8
Figure 7.5 Representation of specimen OLCP_7002 and position of gauges.
Table 7.5 Longitudinal strains in specimen OLCP_7002. Load: 2960 lb (13150 N).
POINT
8
(1
if
(1
1E3
if
1E3
TESTING
THEORY
4_4
3_96
142
X
1 +
Table 7.6 Interlaminar shear strains in specimen OLCP_7002. Load: 2960 lb (13150 N).
POINT
(5 ,. 1E3 TESTING
(5 .. 1E3 THEORY
1
6.0
5.7
3
13.1 (FAI LURE)
12.5
4
11.0
11.6
5
10.0
9.8
7
2.8
2.3
The maximum vertical displacement is reported in Table 7.7. In both fields, strains and displacements, an excellent agreement is found between the data and the prediction.
Table 7.7
Maximum vertical displacement in specimen OLCP_7002. Load: 2960 Ib (13150 N).
POINT
dZ
8
 0.157
d
TESTING
(0.004)
z
THEORY
 0.141
(0.0036)
The scheme of specimen OLCP_7003 is shown in Fig. 7.6. The angle of change of thickness is 90°. Six steps were designed along the specimen. The failure load was 2485 lb (11 046 N). Owing to the fact that the angle of variation of thickness is very high, failure appears at the upper surface in the thinnest area of change of thickness at a low failure load. As occurred with specimen OLCP_7002, failure mechanism is a kind of interlaminar shear mode. As theoretical results predict, there is a remarkable peak of interlaminar shear strains in the places where the thickness changes. The position of the situation of the gauges is shown in Fig. 7.8. The numerical results of the specimen OLCP_7003 are presented in Tables 7.8·7.10. Tables 7.8 and 7.9 show longitudinal and interlaminar shear strains in the critical points for the failure load, respectively. The maximum value is registered in point number 3 (E5=O.0139).
143
0.55(0.014) 0.28(0.007)
I
!
I
0.66(0.0167)
I
14
,0.41 (0.0 1 0) I
I 2.4(0.061 )
I
4.4(0. 111)
'4
,
6.4(0. 162)
,
,
8(0.203)
I
1
I
Figure 7.6 Scheme and measurements of specimen OLCP_7003 in inches (metres).
lP
z
1
11
5
4
3
'x
Ix
IX
x7
1
M
8
Figure 7.7 Representation of specimen OLCP_7003 and position of gauges.
Table 7.8 Longitudinal strains in specimen OLCP_7003. Load: 2485 lb (11046 N).
POINT
8
(1
~
(1
1E3
~
1E3
TESTING
THEORY
5.13
4.6
144
K ~
Table 7.9 Interlaminar shear strains in specimen OLCP_7003. Load: 2485 lb (11 046 N).
POINT
(5
'* 1E3
'* 1E3
(5
THEORY
TESTING
1
7.25
7.5
3
13.9(FAILURE)
12.5
4
12.18
11.6
5
11.02
9.8
7
3.77
3.4
The maximum vertical displacement is reported in Table 7.7. In both fields, strains and displacements, an excellent agreement is found between the data and the prediction. Table 7.10
Maximum vertical displacement in specimen OLCP_7003. Load: 2485 lb (11046 N).
POINT
dZ
8
 0.171
d
TESTING
(0.00432)
z
THEORY
 0.157
(0.004)
Tables 7.11·7.13 show the values of longitudinal, interlaminar shear strains and maxima vertical displacements, respectively, for a load of 1000 Ib (4445 N) for the three specimens. Table 7.11
Longitudinal strains in specimens OLCP_7001, OLCP_7002 and OLCP_7003. Load: 1000 Ib (4445 N).
POINT
8
(1
if
1E3
(1
if
1E3
OLCP_7001
OLCP_7002
1.78
1.77
(1
'* 1E3
OLCP_7003 1.76
As expected, the longitudinal strains at the inner surface in the middle of the span are very similar for the three specimens tested. The reason for this is that the three specimens present the same thickness at the middle of the span and, therefore, the longitudinal strains and stresses are very close in all three cases.
145
Table 7.12. Interlaminar shear strains in specimens OLCP_7001, OLCP_7002 and OLCP_7003. Load: 1000 Ib (4445 N).
POINT
(5
*
1E3
OLCP_7001
(5 * 1E3 OLCP_7002
(5
*
1E3
OLCP_7003
1
2.62
2.5
2.4
3
1.26
4.8
5.24
4
1.14
4.2
4.4
5
0.84
3.8
4.0
7
2.54
1.3
1.12
Table 7.12 shows very good results. On the one hand, the maximum values are registered in specimens OLCP_7002 and OLCP_7003, whose angles of variation of thickness present high values (45° and 90°, respectively). On the other hand, in these two cases, the values given by gauges numbers 3,4 and 5 are critical, which means that the upper surface is the critical one from the failure point of view. However, specimen OLCP_7001 does not present its maximum value in any of these points and, therefore, the tapered surface is not critical at all.
Table 7.13
Maximum vertical displacement in specimens OLCP_7001, OLCP_7002 and OLCP_7003. Load: 1000 Ib (4445 N).
POINT 8
dZ
dZ
OLCP_7001
OLCP_7002
dZ OLCP_7003
 0.0346 (0.00087)  0.059 (0.00149) 0.0628 (0.00159)
The results reported in Table 7.13 highlight the higher stiffness of specimen OLCP_7001 with respect to the other two. The lower the angle of variation of thickness, the better the fibre works. Hence, according to these results, there is no linearity, and the angle of variation of thickness must be very low in order to get a high quality design from the point of view of stiffness and strength. Figures 7.8 and 7.9 can be used to compare the distributions of interlaminar strains through the laminate thickness. Both graphs refer to the threepoint bending test and the specimen OLCP_7001 described above. Figure 7.9 shows the theoretical and experimental distributions of interlaminar shear strain £5 in section AA. As we can see in Fig. 7.10, section AA corresponds to the end of the beam. This section is critical because the laminate thickness is minimum. Figure 7.9 represents the same distributions of £5 in section BB, at the middle of the span (Fig. 7.10). In both cases, theoretical and experimental distributions are very close.
146
20,~
£5
*'
EI Theory • Testing
lE3 10 EI EI EI EI EI EI
EI
o
!:J 1.0
EI ElEI"l
0.8
I
I
I
I
0.6
0.4
0.2
0.0
0.2
22
t Figure 7.8 Distribution of E5 through the thickness in section AA 20,~
Theory • Testing
EI
£5
*'
1 E3 10 
o
22 t
Figure 7.9 Distribution of E5 through the thickness in section BB.
z
T
~p B
A
~A
I
B
Figure 7.10 Representation of sections AA and BB.
147
7.3 Optimisation of variable thickness composite beams The problem analysed here can be formulated by means of the following points: •
The objective is to get the minimum weight structure by using strength as a design criterion.
•
The laminate used is [O]n because it is the optimum for onedimensional laminated composite plates subjected to transverse loads.
•
Two side tapered laminates have been considered.
•
Two kinds of plates have been analysed: • thin plates (l/t» to). • thick plates (l/t« 10).
•
Boundary conditions are restricted to: • simply supported plates. • clamped plates. • cantilever plates.
•
Two types of loading have been applied: • uniform load • point load, at the centre of the beam for simply supported and clamped plates, and at the free end of the plate for cantilever plates.
•
The mesh was composed by 400 nodes.
•
The material used is TIOO1N5208.
In Fig. 7.11 the definition of axis coordinates and the shaded key for onedimensional plates are shown.
148
+
+ thickness
x
 thickness
A
e
I
e
I
e
Figure 7.11 Defmition of axis coordinates and shaded key for onedimensional plates.
7.3.1 Thin plates subjected to a uniform load Optimum thin plates subjected to a uniform load are shown in Fig. 7.13. Whatever the boundary conditions, the optimum laminate thickness is: t = 2k
a (PIX)1I2
[7.1]
where a is the plate span, P is the load applied, X is the uniaxial tensile strength of a ply along the xaxis, and k is a coefficient that varies in function of x. The value of the nondimensional coefficient k in function of x is given for the following boundary conditions: simply supported, clamped and cantilever onedimensional plate. Also, the weight savings (WS) are reported for these three cases. The 45.7 % WS for the cantilever plate is remarkable.
149
111111
~ 111111 ~
WS 24.1 %
k
~111111
WS 38.6 %
WS 45.7 %
k
O+'...&....L...................,............~.........:......&..j 1 o
O+L~~~~~~~~
o
o 2x e
1
2x
e
X
e
Figure 7.12 Representation of optimal thin onedimensional plates subjected to a uniform distributed transverse load.
7.3.2. Thick plates subjected to a uniform load Fig. 7.13 shows the optimum thick plates subjected to a uniform load. In this case, the optimum laminate thickness is: t=
2 k a PIS
[7.2]
where S is the shear strength in the xy or 12plane of a ply. The value of the nondimensional coefficient k is a function of x and the optimum configurations are given for the boundary conditions mentioned above. The weight saving is the same for the three boundary conditions: 45.7 %.
d
111111n
~ 111111 f
WS 45.7 %
p t=2ke
~l!ll!l
WS 45.7 %
p t=2ke
P 5
t=2ke
5
0.5 ~, 0.5 . ,            ,
5
0.5
r. .... 
k
o
o 1
o 2x e
.... I'. .... 1'.
k
k
WS 45.7 %
o 2x
1
8
o
........
~In'h X
e
Figure7.13 Representation of optimal thick onedimensional plates subjected to a uniform distributed transverse load. 150
7.3.3 Thin plates subjected to a point load Optimum thin plates subjected to a point load are shown in Fig. 7.14. Whatever the boundary conditions, the optimum laminate thickness is : t
=2 k
(P aIX)1I2
[7.3]
The value of the nondimensional coefficient k in function of x is given for the following boundary conditions: simply supported, clamped and cantilever onedimensional plate. Also, the weight savings (WS) are reported for these three cases. The 44.0 % WS for clamped plates is remarkable.
1
~tr::!!>h
1
WS 34.5 %
1
WS 44.0 %
WS 37.6 %
t2kjP8 X
~ W!fQ ~
1.2 ,             ,
.
:.0
"0:. .
1.2,, 1.2
r" ....
r . . . k
k
k Of'''........................a...r~.............L....L....L...Ij
o 2>
10); • thick plates (lit < 10).
•
Boundary conditions are restricted to : • simply supported plates along the four edges of the plate. • clamped plates along the four edges of the plate.
•
Two types of loading have been applied: • uniform load; • point load, at the centre of the plate for simply supported and clamped plates, and at the free end of the plate for cantilever plates.
•
The mesh was composed by 400 nodes.
•
The material used is TIOOIN5208.
8.4.1 Thin, simply supponed plates subjected to a uniform load Weight saving and normalised deflection for thin, simply supported, uniform loaded plates are shown in Fig. 8.7. As we can see, the weight saving is a function of the aspect ratio, the maximum value being 27% for a square plate. The optimum sublaminate also varies as a function of the aspect ratio: •
[45/45] for b/a between 1 and 1.75.
•
[0/45/45] for b/a between 1.75 and 2.25.
•
[05/45/45] for b/a between 2.25 and 3.5.
160
•
[0] for b/a higher than 3.5.
WEIGHT SAVI NG (%) Q;so • [45/45]ns • [0/45/45]ns
NORMALIZED DEFLECTION
Deflection tapered plate Deflection untapered plate
EI
[Os/45/45]ns  [O]n A
2 ~~
30
20
10
o
o
2
3
b 4
5
6
o
7
a
2
3 b 4
5
6
7
a
Figure 8.6 Weight saving and normalised deflection for a thin, simply supported plate subjected to a uniform distributed transverse load.
The quasiisotropic sublaminate [0/45/45/90] presents low weight saving with respect to other sublaminates, the maximum value being 18% for a square plate. For thin plates, the optimum laminate thickness can be calculated by means of the following expression: t= 2k
a (PIX)1I2
[8.1]
where a is the length of the plate, P is the load applied, X is the uniaxial tensile strength of a ply along the xaxis, and k is a nondimensional coefficient that is a function of x and y. We can see the values of k along the xaxis and the diagonal in Fig. 8.78.10.
161
b
< e < 1.75 OPTIMUM SUBLAMINATE
[ 45/45]
1.S .,....,
1.S  r           ,
k
k
o+L~~~~~~~
1
o
2
o 2
x
8
X
1
Figure 8.7 Representation of an optimal thin, simply supported plate subjected to a uniform distributed transverse load for aspect ratios between 1 and 1.75.
1.75 ~
eb
< 2.25
OPT IMUM SUBLAM I NATE
[0/45/45]
1.S
r,
1.S
k
k
o ~~~~~~~~ 1 o 2X
o 1
o
2
X
1
8
Figure 8.8 Representation of an optimal thin, simply supported plate subjected to a uniform distributed transverse load for aspect ratios between 1.75 and 2.25.
162
2.25 ~
eb < 3.5
OPTIMUM SUBLAMINATE [OS /45/ 45]
t=2kejf 1.S
~,
1.S
k
k
a ~~~~~~~~ 1 a 2x
a
a
1
2 x
e
1
Figure 8.9 Representation of an optimal thin, simply supported plate subjected to a Wliform distributed transverse load for aspect ratios between 2.25 and 3.5.
b
3.5 ~ e
OPTIMUM SUBLAMINATE [0]
t=2kejf 1.S
~,
K
a
a 2x
1
e Figure 8.10 Representation of an optimal thin, simply supported plate subjected to a uniform distributed transverse load for aspect ratios higher than 3.5.
163
8.4.2 Thin, clamped plates subjected to a uniform load Results for thin, clamped, uniform loaded plates are represented in Fig. 8.12. The weight saving with respect to the constant thickness plate is a function of the aspect ratio, the maximum value being 48% for b/a=2. The optimum sublaminate also varies as a function of the aspect ratio: •
[0/90] for b/a between 1 and 1.5.
•
[05/902] for b/a between 1.5 and 4.4
•
[0] for b/a higher than 4.4
WEIGHT SAYI NG (%)
t:I
Q;so
..
[Os/90z]ns
•
[O/90]ns
•
[O]n
NORMALIZED DEFLECTION
Deflection tapered plate Deflection untapered plate
50 ~~ 40
30 20 10
o
o
2
6 b
8
10
o
12
a
2
4
6 b
8
10
12
a
Figure 8.11 Weight saving and normalised deflection for a thin, clamped plate subjected to a uniform distributed transverse load. The values of the nondimensional parameter k along the xaxis and the diagonal are shown in Fig. 8.128.14.
164
b
< e < 1.5 OPTIMUM SUBLAMINATE [0/90]
0.8..,,
0.8 ,           ,
k
o
k TL.L...L.,,L...L..L..1r...L....LL,.JI....LL
1
o
f
o 2x
o
1
x
2
e
1
Figure 8.12 Representation of an optimal thin, clamped plate subjected to a uniform distributed transverse load for aspect ratios between 1 and 1.5.
1.5 ~
b
e